# Electronic Supplementary Material (ESI) for New Journal of Chemistry.
# This journal is © The Royal Society of Chemistry and the Centre National de la Recherche Scientifique 2020

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_P21N
_database_code_depnum_ccdc_archive 'CCDC 2041200'
loop_
_audit_author_name
_audit_author_address
'ai-quan jia'
;anhui university of technology
China
;
_audit_update_record             
;
2020-10-29 deposited with the CCDC.	2020-12-02 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2016/6
_shelx_SHELXL_version_number     2016/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Cs8 H0 Mo12 Na6 O67 P2 Ru V6'
_chemical_formula_weight         3893.15

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ru Ru -1.2594 0.8363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_H-M_alt        'P 21/n'
_space_group_name_Hall           '-P 2yn'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x+1/2, y+1/2, -z+1/2'
'-x, -y, -z'
'x-1/2, -y-1/2, z-1/2'

_cell_length_a                   13.4946(18)
_cell_length_b                   19.450(3)
_cell_length_c                   17.180(2)
_cell_angle_alpha                90
_cell_angle_beta                 105.833(3)
_cell_angle_gamma                90
_cell_volume                     4338.0(10)
_cell_formula_units_Z            2
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    8576
_cell_measurement_theta_min      2.24
_cell_measurement_theta_max      28.34

_exptl_crystal_description       block
_exptl_crystal_colour            black
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    2.980
_exptl_crystal_F_000             3516
_exptl_transmission_factor_min   0.251
_exptl_transmission_factor_max   0.345
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.20
_exptl_crystal_size_min          0.18
_exptl_absorpt_coefficient_mu    5.919
_shelx_estimated_absorpt_T_min   0.251
_shelx_estimated_absorpt_T_max   0.345
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   sadabs
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            23453
_diffrn_reflns_av_unetI/netI     0.0427
_diffrn_reflns_av_R_equivalents  0.0391
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_theta_min         1.617
_diffrn_reflns_theta_max         24.999
_diffrn_reflns_theta_full        24.999
_diffrn_measured_fraction_theta_max 0.989
_diffrn_measured_fraction_theta_full 0.989
_diffrn_reflns_Laue_measured_fraction_max 0.989
_diffrn_reflns_Laue_measured_fraction_full 0.989
_diffrn_reflns_point_group_measured_fraction_max 0.989
_diffrn_reflns_point_group_measured_fraction_full 0.989
_reflns_number_total             7544
_reflns_number_gt                6123
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_max     .
_reflns_Friedel_fraction_full    .

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker SMART'
_computing_cell_refinement       'Bruker SMART'
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          ?
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0100P)²+240.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_extinction_coef       0.00035(4)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_number_reflns         7544
_refine_ls_number_parameters     476
_refine_ls_number_restraints     1149
_refine_ls_R_factor_all          0.0969
_refine_ls_R_factor_gt           0.0823
_refine_ls_wR_factor_ref         0.1946
_refine_ls_wR_factor_gt          0.1893
_refine_ls_goodness_of_fit_ref   1.214
_refine_ls_restrained_S_all      1.239
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ru1 Ru 0.000000 1.000000 1.000000 0.0283(4) Uani 1 2 d S U P . .
Mo1 Mo -0.11494(12) 0.69527(7) 1.01333(9) 0.0324(4) Uani 1 1 d . U . . .
Mo2 Mo -0.13769(11) 0.77175(7) 0.79980(8) 0.0260(3) Uani 1 1 d . U . . .
Mo3 Mo 0.08136(12) 0.82450(7) 0.76435(9) 0.0311(4) Uani 1 1 d . U . . .
Mo4 Mo 0.32955(12) 0.80466(9) 0.93959(14) 0.0495(5) Uani 1 1 d . U . . .
Mo5 Mo 0.20349(13) 0.64546(8) 0.82989(12) 0.0427(4) Uani 1 1 d . U . . .
Mo6 Mo -0.01487(12) 0.59147(7) 0.86482(10) 0.0337(4) Uani 1 1 d . U . . .
V1 V -0.1821(2) 1.06770(14) 1.09507(19) 0.0333(7) Uani 1 1 d . U . . .
V2 V -0.1532(2) 0.84968(14) 0.96040(18) 0.0295(6) Uani 1 1 d . U . . .
V3 V -0.0786(2) 0.94271(13) 0.81547(17) 0.0271(6) Uani 1 1 d . U . . .
Cs1 Cs 0.14833(13) 0.59117(8) 1.10701(11) 0.0692(5) Uani 1 1 d . U . . .
Cs2 Cs -0.20411(17) 1.13854(9) 0.86693(10) 0.0849(6) Uani 1 1 d . U . . .
Cs3 Cs 0.14608(15) 0.72135(11) 0.57912(13) 0.0850(6) Uani 1 1 d . U . . .
Cs4 Cs 0.3233(3) 0.93213(15) 0.6974(3) 0.1795(16) Uani 1 1 d . U . . .
Na1 Na 0.0883(7) 0.7479(6) 0.3340(7) 0.077(3) Uani 1 1 d . U . . .
P1 P 0.0915(3) 0.7457(2) 0.9472(3) 0.0267(8) Uani 1 1 d . U . . .
O1 O -0.2265(11) 0.9992(7) 1.1259(9) 0.054(3) Uani 1 1 d . U . . .
O2 O -0.1149(10) 1.0461(6) 1.0278(8) 0.041(2) Uani 1 1 d . U . . .
O3 O 0.0640(10) 1.0901(6) 0.9972(7) 0.040(2) Uani 1 1 d . U . . .
O4 O -0.0723(9) 1.0091(6) 0.8794(7) 0.0366(18) Uani 1 1 d . U . . .
O5 O -0.1442(9) 0.9698(6) 0.7275(7) 0.038(2) Uani 1 1 d . U . . .
O6 O 0.0525(9) 0.9229(6) 0.8152(8) 0.0363(16) Uani 1 1 d . U . . .
O7 O -0.1458(9) 0.8739(6) 0.8480(7) 0.0342(15) Uani 1 1 d . U . . .
O8 O -0.2665(10) 0.8786(7) 0.9544(8) 0.044(2) Uani 1 1 d . U . . .
O9 O -0.1341(9) 0.7871(6) 1.0457(7) 0.0364(17) Uani 1 1 d . U . . .
O10 O -0.1628(9) 0.7598(6) 0.9024(7) 0.0338(15) Uani 1 1 d . U . . .
O11 O -0.2597(9) 0.7762(6) 0.7346(8) 0.038(2) Uani 1 1 d . U . . .
O12 O -0.0672(9) 0.8225(6) 0.7335(8) 0.0367(15) Uani 1 1 d . U . . .
O13 O 0.0969(11) 0.8588(7) 0.6768(9) 0.0491(19) Uani 1 1 d . U . . .
O14 O 0.2044(10) 0.8502(6) 0.8424(9) 0.0448(16) Uani 1 1 d . U . . .
O15 O 0.2994(10) 0.8926(7) 0.9762(9) 0.048(2) Uani 1 1 d . U . . .
O16 O 0.4190(11) 0.8295(8) 0.8895(12) 0.066(2) Uani 1 1 d . U . . .
O17 O 0.4058(11) 0.7697(8) 1.0250(11) 0.062(2) Uani 1 1 d . U . . .
O18 O 0.1953(9) 0.7768(6) 0.9820(8) 0.0423(17) Uani 1 1 d . U . . .
O19 O 0.0285(9) 0.7902(6) 0.8765(7) 0.0343(14) Uani 1 1 d . U . . .
O20 O 0.0349(9) 0.7384(6) 1.0111(8) 0.0356(16) Uani 1 1 d . U . . .
O21 O -0.0980(9) 0.6882(6) 0.7897(8) 0.0364(16) Uani 1 1 d . U . . .
O22 O -0.2407(10) 0.6661(6) 0.9970(8) 0.042(2) Uani 1 1 d . U . . .
O23 O -0.0546(10) 0.6590(6) 1.1050(8) 0.0422(19) Uani 1 1 d . U . . .
O24 O -0.0786(9) 0.6315(6) 0.9381(8) 0.0376(15) Uani 1 1 d . U . . .
O25 O 0.1062(9) 0.6735(6) 0.9128(8) 0.0380(14) Uani 1 1 d . U . . .
O26 O 0.1124(10) 0.7383(6) 0.7574(8) 0.0413(15) Uani 1 1 d . U . . .
O27 O 0.2858(10) 0.7211(7) 0.8773(9) 0.0477(16) Uani 1 1 d . U . . .
O28 O 0.2443(11) 0.6332(7) 0.7453(10) 0.052(2) Uani 1 1 d . U . . .
O29 O 0.2657(11) 0.5821(7) 0.8915(9) 0.050(2) Uani 1 1 d . U . . .
O30 O 0.0684(10) 0.6011(6) 0.7894(8) 0.0422(16) Uani 1 1 d . U . . .
O31 O 0.0537(10) 0.5284(6) 0.9244(9) 0.0465(19) Uani 1 1 d . U . . .
O32 O -0.1145(10) 0.5469(6) 0.8016(8) 0.044(2) Uani 1 1 d . U . . .
O34 O -0.335(2) 1.0004(14) 0.8585(16) 0.046(3) Uani 0.5 1 d . U P . .
Na4 Na 0.0559(9) 1.1221(8) 0.8014(7) 0.106(4) Uani 1 1 d . U . . .
Na3 Na 0.4408(11) 0.9524(8) 1.0695(13) 0.150(7) Uani 1 1 d . U . . .
O74 O 0.262(2) 0.4785(14) 1.018(2) 0.059(4) Uani 0.5 1 d . U P . .
O78 O 0.418(2) 0.998(2) 0.825(3) 0.094(5) Uani 0.5 1 d . U P . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ru1 O2 1.959(13) 3_577 ?
Ru1 O2 1.959(13) . ?
Ru1 O3 1.960(12) 3_577 ?
Ru1 O3 1.960(12) . ?
Ru1 O4 2.042(12) 3_577 ?
Ru1 O4 2.043(12) . ?
Ru1 Cs2 4.0789(16) 3_577 ?
Mo1 O23 1.715(13) . ?
Mo1 O22 1.738(13) . ?
Mo1 O9 1.910(12) . ?
Mo1 O24 1.948(12) . ?
Mo1 O20 2.198(12) . ?
Mo1 O10 2.226(12) . ?
Mo1 V2 3.140(3) . ?
Mo1 Cs3 4.037(2) 4_576 ?
Mo1 Cs4 4.275(4) 4_576 ?
Mo2 O11 1.723(12) . ?
Mo2 O21 1.734(11) . ?
Mo2 O10 1.898(12) . ?
Mo2 O12 1.941(12) . ?
Mo2 O7 2.167(11) . ?
Mo2 O19 2.299(12) . ?
Mo2 Cs2 4.017(2) 2_446 ?
Mo3 O13 1.709(14) . ?
Mo3 O26 1.740(12) . ?
Mo3 O14 1.894(14) . ?
Mo3 O12 1.929(12) . ?
Mo3 O6 2.184(12) . ?
Mo3 O19 2.328(12) . ?
Mo4 O17 1.688(16) . ?
Mo4 O16 1.732(16) . ?
Mo4 O15 1.904(13) . ?
Mo4 O27 1.947(14) . ?
Mo4 O18 2.197(13) . ?
Mo4 O14 2.210(13) . ?
Mo4 V1 3.135(3) 3_577 ?
Mo4 Na3 3.696(13) . ?
Mo4 Cs2 4.267(3) 3_577 ?
Mo4 Cs3 4.320(3) 4_676 ?
Mo5 O29 1.691(14) . ?
Mo5 O28 1.705(15) . ?
Mo5 O27 1.889(14) . ?
Mo5 O30 1.965(13) . ?
Mo5 O25 2.253(12) . ?
Mo5 O26 2.342(13) . ?
Mo5 Cs4 4.180(3) 2_546 ?
Mo6 O31 1.701(13) . ?
Mo6 O32 1.715(13) . ?
Mo6 O24 1.877(12) . ?
Mo6 O30 1.942(13) . ?
Mo6 O25 2.271(12) . ?
Mo6 O21 2.382(12) . ?
Mo6 Cs1 4.071(2) 3_567 ?
Mo6 Cs4 4.352(3) 2_546 ?
V1 O1 1.609(13) . ?
V1 O2 1.705(13) . ?
V1 O15 1.882(14) 3_577 ?
V1 O14 1.993(13) 3_577 ?
V1 O6 1.999(13) 3_577 ?
V2 O8 1.605(13) . ?
V2 O3 1.695(12) 3_577 ?
V2 O9 1.867(12) . ?
V2 O10 1.998(12) . ?
V2 O7 2.016(12) . ?
V2 Cs3 4.052(3) 4_576 ?
V3 O5 1.617(12) . ?
V3 O4 1.682(12) . ?
V3 O7 1.789(12) . ?
V3 O6 1.811(12) . ?
V3 Cs2 4.356(3) . ?
V3 Cs1 4.431(3) 4_575 ?
Cs1 O23 3.031(13) . ?
Cs1 O32 3.205(13) 3_567 ?
Cs1 O5 3.220(12) 4_676 ?
Cs1 O74 3.28(3) . ?
Cs1 O31 3.282(15) . ?
Cs1 O11 3.393(12) 4_676 ?
Cs1 O20 3.447(12) . ?
Cs1 O31 3.512(13) 3_567 ?
Cs1 O25 3.602(13) . ?
Cs1 O24 3.683(13) . ?
Cs2 O18 3.049(14) 3_577 ?
Cs2 O4 3.057(11) . ?
Cs2 O11 3.160(12) 2_456 ?
Cs2 O34 3.20(3) . ?
Cs2 O2 3.241(13) . ?
Cs2 O15 3.342(15) 3_577 ?
Cs2 O21 3.375(12) 2_456 ?
Cs2 O20 3.567(12) 3_577 ?
Cs2 O32 3.700(14) 2_456 ?
Cs2 P1 3.864(5) 3_577 ?
Cs2 Na4 3.979(14) . ?
Cs3 O17 3.124(14) 4_575 ?
Cs3 O9 3.176(12) 4_675 ?
Cs3 O22 3.209(13) 4_675 ?
Cs3 O26 3.234(13) . ?
Cs3 O28 3.284(16) . ?
Cs3 O13 3.318(14) . ?
Cs3 O8 3.338(14) 4_675 ?
Cs3 Na1 4.101(12) . ?
Cs3 Na3 4.344(16) 4_575 ?
Cs4 O78 2.56(5) . ?
Cs4 O23 3.131(13) 4_675 ?
Cs4 O13 3.303(15) . ?
Cs4 O29 3.358(14) 2_556 ?
Cs4 O31 3.541(14) 2_556 ?
Cs4 O30 3.578(12) 2_556 ?
Cs4 O74 3.67(3) 2_556 ?
Cs4 O14 3.675(14) . ?
Cs4 O16 3.770(19) . ?
Na1 Na4 3.622(17) 3_576 ?
P1 O18 1.493(13) . ?
P1 O20 1.507(13) . ?
P1 O19 1.544(12) . ?
P1 O25 1.557(12) . ?
O15 Na3 2.428(19) . ?
O34 Na3 2.32(3) 3_577 ?
Na3 O78 2.44(5) 3_677 ?
Na3 Na3 3.71(4) 3_677 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O2 Ru1 O2 180.0 3_577 . ?
O2 Ru1 O3 88.9(5) 3_577 3_577 ?
O2 Ru1 O3 91.1(5) . 3_577 ?
O2 Ru1 O3 91.1(5) 3_577 . ?
O2 Ru1 O3 88.9(5) . . ?
O3 Ru1 O3 180.0 3_577 . ?
O2 Ru1 O4 91.0(5) 3_577 3_577 ?
O2 Ru1 O4 89.0(5) . 3_577 ?
O3 Ru1 O4 89.4(5) 3_577 3_577 ?
O3 Ru1 O4 90.6(5) . 3_577 ?
O2 Ru1 O4 89.0(5) 3_577 . ?
O2 Ru1 O4 91.0(5) . . ?
O3 Ru1 O4 90.6(5) 3_577 . ?
O3 Ru1 O4 89.4(5) . . ?
O4 Ru1 O4 180.0 3_577 . ?
O2 Ru1 Cs2 51.4(4) 3_577 3_577 ?
O2 Ru1 Cs2 128.6(4) . 3_577 ?
O3 Ru1 Cs2 68.3(4) 3_577 3_577 ?
O3 Ru1 Cs2 111.7(4) . 3_577 ?
O4 Ru1 Cs2 46.5(3) 3_577 3_577 ?
O4 Ru1 Cs2 133.5(3) . 3_577 ?
O23 Mo1 O22 102.3(6) . . ?
O23 Mo1 O9 100.7(6) . . ?
O22 Mo1 O9 98.6(6) . . ?
O23 Mo1 O24 101.8(6) . . ?
O22 Mo1 O24 95.5(6) . . ?
O9 Mo1 O24 150.2(5) . . ?
O23 Mo1 O20 87.9(5) . . ?
O22 Mo1 O20 169.6(5) . . ?
O9 Mo1 O20 81.1(5) . . ?
O24 Mo1 O20 80.4(5) . . ?
O23 Mo1 O10 166.5(5) . . ?
O22 Mo1 O10 90.2(5) . . ?
O9 Mo1 O10 72.0(5) . . ?
O24 Mo1 O10 81.8(5) . . ?
O20 Mo1 O10 79.8(4) . . ?
O23 Mo1 V2 131.2(4) . . ?
O22 Mo1 V2 100.9(4) . . ?
O9 Mo1 V2 33.3(4) . . ?
O24 Mo1 V2 117.9(4) . . ?
O20 Mo1 V2 73.1(3) . . ?
O10 Mo1 V2 39.3(3) . . ?
O23 Mo1 Cs3 97.1(4) . 4_576 ?
O22 Mo1 Cs3 50.0(4) . 4_576 ?
O9 Mo1 Cs3 50.3(4) . 4_576 ?
O24 Mo1 Cs3 143.7(4) . 4_576 ?
O20 Mo1 Cs3 131.3(3) . 4_576 ?
O10 Mo1 Cs3 86.9(3) . 4_576 ?
V2 Mo1 Cs3 67.41(7) . 4_576 ?
O23 Mo1 Cs4 38.9(4) . 4_576 ?
O22 Mo1 Cs4 63.4(4) . 4_576 ?
O9 Mo1 Cs4 105.0(4) . 4_576 ?
O24 Mo1 Cs4 104.9(4) . 4_576 ?
O20 Mo1 Cs4 126.8(3) . 4_576 ?
O10 Mo1 Cs4 153.0(3) . 4_576 ?
V2 Mo1 Cs4 135.96(8) . 4_576 ?
Cs3 Mo1 Cs4 72.18(5) 4_576 4_576 ?
O11 Mo2 O21 104.4(6) . . ?
O11 Mo2 O10 103.3(6) . . ?
O21 Mo2 O10 96.7(5) . . ?
O11 Mo2 O12 97.3(6) . . ?
O21 Mo2 O12 101.7(5) . . ?
O10 Mo2 O12 147.9(5) . . ?
O11 Mo2 O7 93.6(5) . . ?
O21 Mo2 O7 161.2(5) . . ?
O10 Mo2 O7 73.5(5) . . ?
O12 Mo2 O7 80.9(5) . . ?
O11 Mo2 O19 167.2(5) . . ?
O21 Mo2 O19 85.6(5) . . ?
O10 Mo2 O19 83.1(5) . . ?
O12 Mo2 O19 72.5(5) . . ?
O7 Mo2 O19 77.3(4) . . ?
O11 Mo2 Cs2 48.8(4) . 2_446 ?
O21 Mo2 Cs2 56.2(4) . 2_446 ?
O10 Mo2 Cs2 112.9(4) . 2_446 ?
O12 Mo2 Cs2 99.2(4) . 2_446 ?
O7 Mo2 Cs2 142.3(3) . 2_446 ?
O19 Mo2 Cs2 139.1(3) . 2_446 ?
O13 Mo3 O26 103.1(6) . . ?
O13 Mo3 O14 103.1(7) . . ?
O26 Mo3 O14 97.0(6) . . ?
O13 Mo3 O12 97.7(6) . . ?
O26 Mo3 O12 102.3(5) . . ?
O14 Mo3 O12 147.5(5) . . ?
O13 Mo3 O6 95.1(6) . . ?
O26 Mo3 O6 160.9(6) . . ?
O14 Mo3 O6 72.7(5) . . ?
O12 Mo3 O6 80.9(5) . . ?
O13 Mo3 O19 168.2(5) . . ?
O26 Mo3 O19 85.1(5) . . ?
O14 Mo3 O19 84.1(5) . . ?
O12 Mo3 O19 72.0(5) . . ?
O6 Mo3 O19 77.9(4) . . ?
O17 Mo4 O16 101.6(8) . . ?
O17 Mo4 O15 102.1(7) . . ?
O16 Mo4 O15 98.9(7) . . ?
O17 Mo4 O27 99.4(7) . . ?
O16 Mo4 O27 96.2(7) . . ?
O15 Mo4 O27 150.6(6) . . ?
O17 Mo4 O18 88.6(7) . . ?
O16 Mo4 O18 169.6(7) . . ?
O15 Mo4 O18 80.9(5) . . ?
O27 Mo4 O18 79.8(5) . . ?
O17 Mo4 O14 167.6(7) . . ?
O16 Mo4 O14 90.3(7) . . ?
O15 Mo4 O14 72.6(5) . . ?
O27 Mo4 O14 82.2(5) . . ?
O18 Mo4 O14 79.6(5) . . ?
O17 Mo4 V1 133.5(6) . 3_577 ?
O16 Mo4 V1 100.2(5) . 3_577 ?
O15 Mo4 V1 33.9(4) . 3_577 ?
O27 Mo4 V1 118.4(4) . 3_577 ?
O18 Mo4 V1 73.8(3) . 3_577 ?
O14 Mo4 V1 39.2(3) . 3_577 ?
O17 Mo4 Na3 74.8(6) . . ?
O16 Mo4 Na3 81.9(6) . . ?
O15 Mo4 Na3 36.0(5) . . ?
O27 Mo4 Na3 173.3(5) . . ?
O18 Mo4 Na3 103.2(5) . . ?
O14 Mo4 Na3 104.2(5) . . ?
V1 Mo4 Na3 68.4(3) 3_577 . ?
O17 Mo4 Cs2 72.8(6) . 3_577 ?
O16 Mo4 Cs2 142.5(6) . 3_577 ?
O15 Mo4 Cs2 49.0(4) . 3_577 ?
O27 Mo4 Cs2 121.3(4) . 3_577 ?
O18 Mo4 Cs2 42.9(4) . 3_577 ?
O14 Mo4 Cs2 95.8(4) . 3_577 ?
V1 Mo4 Cs2 64.97(7) 3_577 3_577 ?
Na3 Mo4 Cs2 60.7(3) . 3_577 ?
O17 Mo4 Cs3 36.3(5) . 4_676 ?
O16 Mo4 Cs3 65.8(6) . 4_676 ?
O15 Mo4 Cs3 101.0(4) . 4_676 ?
O27 Mo4 Cs3 108.2(4) . 4_676 ?
O18 Mo4 Cs3 124.5(4) . 4_676 ?
O14 Mo4 Cs3 154.5(3) . 4_676 ?
V1 Mo4 Cs3 132.71(8) 3_577 4_676 ?
Na3 Mo4 Cs3 65.1(3) . 4_676 ?
Cs2 Mo4 Cs3 98.07(6) 3_577 4_676 ?
O29 Mo5 O28 102.1(7) . . ?
O29 Mo5 O27 99.5(6) . . ?
O28 Mo5 O27 100.8(6) . . ?
O29 Mo5 O30 98.9(6) . . ?
O28 Mo5 O30 97.0(6) . . ?
O27 Mo5 O30 151.0(5) . . ?
O29 Mo5 O25 93.2(6) . . ?
O28 Mo5 O25 162.3(6) . . ?
O27 Mo5 O25 85.1(5) . . ?
O30 Mo5 O25 71.7(5) . . ?
O29 Mo5 O26 173.5(6) . . ?
O28 Mo5 O26 84.2(6) . . ?
O27 Mo5 O26 77.9(5) . . ?
O30 Mo5 O26 81.3(5) . . ?
O25 Mo5 O26 80.7(4) . . ?
O29 Mo5 Cs4 50.2(5) . 2_546 ?
O28 Mo5 Cs4 78.7(5) . 2_546 ?
O27 Mo5 Cs4 147.6(4) . 2_546 ?
O30 Mo5 Cs4 58.7(4) . 2_546 ?
O25 Mo5 Cs4 105.3(3) . 2_546 ?
O26 Mo5 Cs4 133.5(3) . 2_546 ?
O31 Mo6 O32 102.7(6) . . ?
O31 Mo6 O24 99.7(6) . . ?
O32 Mo6 O24 102.2(6) . . ?
O31 Mo6 O30 98.7(6) . . ?
O32 Mo6 O30 97.0(6) . . ?
O24 Mo6 O30 149.6(5) . . ?
O31 Mo6 O25 93.9(6) . . ?
O32 Mo6 O25 161.3(6) . . ?
O24 Mo6 O25 83.2(5) . . ?
O30 Mo6 O25 71.6(5) . . ?
O31 Mo6 O21 173.9(6) . . ?
O32 Mo6 O21 83.4(5) . . ?
O24 Mo6 O21 78.5(5) . . ?
O30 Mo6 O21 80.5(5) . . ?
O25 Mo6 O21 80.1(4) . . ?
O31 Mo6 Cs1 59.0(4) . 3_567 ?
O32 Mo6 Cs1 48.6(4) . 3_567 ?
O24 Mo6 Cs1 89.1(4) . 3_567 ?
O30 Mo6 Cs1 121.2(4) . 3_567 ?
O25 Mo6 Cs1 150.2(3) . 3_567 ?
O21 Mo6 Cs1 126.6(3) . 3_567 ?
O31 Mo6 Cs4 51.1(5) . 2_546 ?
O32 Mo6 Cs4 84.2(4) . 2_546 ?
O24 Mo6 Cs4 150.7(4) . 2_546 ?
O30 Mo6 Cs4 54.1(4) . 2_546 ?
O25 Mo6 Cs4 100.0(3) . 2_546 ?
O21 Mo6 Cs4 130.8(3) . 2_546 ?
Cs1 Mo6 Cs4 73.70(5) 3_567 2_546 ?
O1 V1 O2 109.5(7) . . ?
O1 V1 O15 103.4(7) . 3_577 ?
O2 V1 O15 99.7(6) . 3_577 ?
O1 V1 O14 111.2(7) . 3_577 ?
O2 V1 O14 138.5(6) . 3_577 ?
O15 V1 O14 78.3(6) 3_577 3_577 ?
O1 V1 O6 98.5(6) . 3_577 ?
O2 V1 O6 91.7(6) . 3_577 ?
O15 V1 O6 150.2(5) 3_577 3_577 ?
O14 V1 O6 75.0(5) 3_577 3_577 ?
O1 V1 Mo4 116.4(6) . 3_577 ?
O2 V1 Mo4 119.6(4) . 3_577 ?
O15 V1 Mo4 34.3(4) 3_577 3_577 ?
O14 V1 Mo4 44.5(4) 3_577 3_577 ?
O6 V1 Mo4 116.8(3) 3_577 3_577 ?
O8 V2 O3 109.7(7) . 3_577 ?
O8 V2 O9 101.8(6) . . ?
O3 V2 O9 100.5(6) 3_577 . ?
O8 V2 O10 110.1(6) . . ?
O3 V2 O10 139.5(6) 3_577 . ?
O9 V2 O10 78.3(5) . . ?
O8 V2 O7 98.7(6) . . ?
O3 V2 O7 92.0(6) 3_577 . ?
O9 V2 O7 150.6(5) . . ?
O10 V2 O7 75.0(5) . . ?
O8 V2 Mo1 115.6(5) . . ?
O3 V2 Mo1 119.7(4) 3_577 . ?
O9 V2 Mo1 34.2(4) . . ?
O10 V2 Mo1 44.8(3) . . ?
O7 V2 Mo1 117.0(3) . . ?
O8 V2 Cs3 52.9(5) . 4_576 ?
O3 V2 Cs3 120.9(5) 3_577 4_576 ?
O9 V2 Cs3 49.6(4) . 4_576 ?
O10 V2 Cs3 89.5(3) . 4_576 ?
O7 V2 Cs3 140.9(4) . 4_576 ?
Mo1 V2 Cs3 66.91(7) . 4_576 ?
O5 V3 O4 106.1(6) . . ?
O5 V3 O7 110.0(6) . . ?
O4 V3 O7 108.0(6) . . ?
O5 V3 O6 110.7(6) . . ?
O4 V3 O6 106.8(6) . . ?
O7 V3 O6 114.9(5) . . ?
O5 V3 Cs2 76.2(4) . . ?
O4 V3 Cs2 31.8(4) . . ?
O7 V3 Cs2 109.4(4) . . ?
O6 V3 Cs2 128.3(4) . . ?
O5 V3 Cs1 34.0(4) . 4_575 ?
O4 V3 Cs1 121.7(4) . 4_575 ?
O7 V3 Cs1 76.2(4) . 4_575 ?
O6 V3 Cs1 124.3(4) . 4_575 ?
Cs2 V3 Cs1 90.60(6) . 4_575 ?
O23 Cs1 O32 97.0(3) . 3_567 ?
O23 Cs1 O5 142.4(3) . 4_676 ?
O32 Cs1 O5 65.9(3) 3_567 4_676 ?
O23 Cs1 O74 145.1(6) . . ?
O32 Cs1 O74 79.4(6) 3_567 . ?
O5 Cs1 O74 67.7(6) 4_676 . ?
O23 Cs1 O31 92.1(3) . . ?
O32 Cs1 O31 95.0(3) 3_567 . ?
O5 Cs1 O31 121.4(3) 4_676 . ?
O74 Cs1 O31 54.2(6) . . ?
O23 Cs1 O11 81.2(3) . 4_676 ?
O32 Cs1 O11 113.4(3) 3_567 4_676 ?
O5 Cs1 O11 76.4(3) 4_676 4_676 ?
O74 Cs1 O11 132.4(6) . 4_676 ?
O31 Cs1 O11 151.4(3) . 4_676 ?
O23 Cs1 O20 49.5(3) . . ?
O32 Cs1 O20 145.7(3) 3_567 . ?
O5 Cs1 O20 143.9(3) 4_676 . ?
O74 Cs1 O20 122.3(6) . . ?
O31 Cs1 O20 81.1(3) . . ?
O11 Cs1 O20 73.4(3) 4_676 . ?
O23 Cs1 O31 68.0(3) . 3_567 ?
O32 Cs1 O31 46.5(3) 3_567 3_567 ?
O5 Cs1 O31 110.9(3) 4_676 3_567 ?
O74 Cs1 O31 85.8(6) . 3_567 ?
O31 Cs1 O31 61.5(4) . 3_567 ?
O11 Cs1 O31 137.3(3) 4_676 3_567 ?
O20 Cs1 O31 104.6(3) . 3_567 ?
O23 Cs1 O25 83.2(3) . . ?
O32 Cs1 O25 144.9(3) 3_567 . ?
O5 Cs1 O25 130.5(3) 4_676 . ?
O74 Cs1 O25 80.8(6) . . ?
O31 Cs1 O25 50.1(3) . . ?
O11 Cs1 O25 101.4(3) 4_676 . ?
O20 Cs1 O25 41.5(3) . . ?
O31 Cs1 O25 103.4(3) 3_567 . ?
O23 Cs1 O24 49.0(3) . . ?
O32 Cs1 O24 111.4(3) 3_567 . ?
O5 Cs1 O24 167.2(3) 4_676 . ?
O74 Cs1 O24 99.7(6) . . ?
O31 Cs1 O24 45.8(3) . . ?
O11 Cs1 O24 115.2(3) 4_676 . ?
O20 Cs1 O24 44.0(3) . . ?
O31 Cs1 O24 64.9(3) 3_567 . ?
O25 Cs1 O24 44.6(3) . . ?
O23 Cs1 Mo6 87.3(2) . 3_567 ?
O32 Cs1 Mo6 23.7(2) 3_567 3_567 ?
O5 Cs1 Mo6 86.4(2) 4_676 3_567 ?
O74 Cs1 Mo6 75.6(5) . 3_567 ?
O31 Cs1 Mo6 73.7(2) . 3_567 ?
O11 Cs1 Mo6 133.0(2) 4_676 3_567 ?
O20 Cs1 Mo6 128.9(2) . 3_567 ?
O31 Cs1 Mo6 24.5(2) 3_567 3_567 ?
O25 Cs1 Mo6 122.3(2) . 3_567 ?
O24 Cs1 Mo6 88.84(18) . 3_567 ?
O23 Cs1 V3 128.5(3) . 4_676 ?
O32 Cs1 V3 71.2(2) 3_567 4_676 ?
O5 Cs1 V3 16.3(2) 4_676 4_676 ?
O74 Cs1 V3 83.5(5) . 4_676 ?
O31 Cs1 V3 137.6(2) . 4_676 ?
O11 Cs1 V3 60.9(2) 4_676 4_676 ?
O20 Cs1 V3 132.3(2) . 4_676 ?
O31 Cs1 V3 117.7(2) 3_567 4_676 ?
O25 Cs1 V3 134.5(2) . 4_676 ?
O24 Cs1 V3 176.13(19) . 4_676 ?
Mo6 Cs1 V3 94.10(5) 3_567 4_676 ?
O18 Cs2 O4 119.9(3) 3_577 . ?
O18 Cs2 O11 88.6(3) 3_577 2_456 ?
O4 Cs2 O11 137.4(3) . 2_456 ?
O18 Cs2 O34 112.7(5) 3_577 . ?
O4 Cs2 O34 67.3(5) . . ?
O11 Cs2 O34 133.4(5) 2_456 . ?
O18 Cs2 O2 69.8(3) 3_577 . ?
O4 Cs2 O2 53.8(3) . . ?
O11 Cs2 O2 155.0(3) 2_456 . ?
O34 Cs2 O2 69.2(5) . . ?
O18 Cs2 O15 49.1(3) 3_577 3_577 ?
O4 Cs2 O15 98.0(3) . 3_577 ?
O11 Cs2 O15 124.3(3) 2_456 3_577 ?
O34 Cs2 O15 63.6(5) . 3_577 ?
O2 Cs2 O15 49.2(3) . 3_577 ?
O18 Cs2 O21 111.3(3) 3_577 2_456 ?
O4 Cs2 O21 127.6(3) . 2_456 ?
O11 Cs2 O21 49.3(3) 2_456 2_456 ?
O34 Cs2 O21 84.1(5) . 2_456 ?
O2 Cs2 O21 150.2(3) . 2_456 ?
O15 Cs2 O21 107.5(3) 3_577 2_456 ?
O18 Cs2 O20 42.9(3) 3_577 3_577 ?
O4 Cs2 O20 104.2(3) . 3_577 ?
O11 Cs2 O20 74.5(3) 2_456 3_577 ?
O34 Cs2 O20 148.0(5) . 3_577 ?
O2 Cs2 O20 80.9(3) . 3_577 ?
O15 Cs2 O20 88.5(3) 3_577 3_577 ?
O21 Cs2 O20 121.1(3) 2_456 3_577 ?
O18 Cs2 O32 142.2(3) 3_577 2_456 ?
O4 Cs2 O32 84.6(3) . 2_456 ?
O11 Cs2 O32 90.4(3) 2_456 2_456 ?
O34 Cs2 O32 47.2(5) . 2_456 ?
O2 Cs2 O32 114.4(3) . 2_456 ?
O15 Cs2 O32 103.0(3) 3_577 2_456 ?
O21 Cs2 O32 45.8(3) 2_456 2_456 ?
O20 Cs2 O32 164.6(3) 3_577 2_456 ?
O18 Cs2 P1 21.0(2) 3_577 3_577 ?
O4 Cs2 P1 109.4(2) . 3_577 ?
O11 Cs2 P1 85.9(2) 2_456 3_577 ?
O34 Cs2 P1 128.0(5) . 3_577 ?
O2 Cs2 P1 69.4(2) . 3_577 ?
O15 Cs2 P1 65.8(2) 3_577 3_577 ?
O21 Cs2 P1 122.6(2) 2_456 3_577 ?
O20 Cs2 P1 23.0(2) 3_577 3_577 ?
O32 Cs2 P1 162.7(2) 2_456 3_577 ?
O18 Cs2 Na4 116.8(3) 3_577 . ?
O4 Cs2 Na4 54.0(3) . . ?
O11 Cs2 Na4 85.9(3) 2_456 . ?
O34 Cs2 Na4 116.0(5) . . ?
O2 Cs2 Na4 92.6(3) . . ?
O15 Cs2 Na4 140.9(3) 3_577 . ?
O21 Cs2 Na4 111.4(3) 2_456 . ?
O20 Cs2 Na4 75.4(3) 3_577 . ?
O32 Cs2 Na4 100.7(3) 2_456 . ?
P1 Cs2 Na4 95.9(2) 3_577 . ?
O18 Cs2 Mo2 98.5(2) 3_577 2_456 ?
O4 Cs2 Mo2 140.1(2) . 2_456 ?
O11 Cs2 Mo2 24.2(2) 2_456 2_456 ?
O34 Cs2 Mo2 109.3(5) . 2_456 ?
O2 Cs2 Mo2 165.3(2) . 2_456 ?
O15 Cs2 Mo2 116.4(2) 3_577 2_456 ?
O21 Cs2 Mo2 25.27(19) 2_456 2_456 ?
O20 Cs2 Mo2 96.68(19) 3_577 2_456 ?
O32 Cs2 Mo2 69.11(19) 2_456 2_456 ?
P1 Cs2 Mo2 103.06(7) 3_577 2_456 ?
Na4 Cs2 Mo2 100.85(18) . 2_456 ?
O17 Cs3 O9 153.3(4) 4_575 4_675 ?
O17 Cs3 O22 114.3(4) 4_575 4_675 ?
O9 Cs3 O22 51.4(3) 4_675 4_675 ?
O17 Cs3 O26 82.7(4) 4_575 . ?
O9 Cs3 O26 123.8(3) 4_675 . ?
O22 Cs3 O26 123.6(3) 4_675 . ?
O17 Cs3 O28 115.3(4) 4_575 . ?
O9 Cs3 O28 87.4(3) 4_675 . ?
O22 Cs3 O28 127.7(3) 4_675 . ?
O26 Cs3 O28 50.0(3) . . ?
O17 Cs3 O13 76.8(4) 4_575 . ?
O9 Cs3 O13 117.3(3) 4_675 . ?
O22 Cs3 O13 81.8(3) 4_675 . ?
O26 Cs3 O13 48.7(3) . . ?
O28 Cs3 O13 94.0(3) . . ?
O17 Cs3 O8 111.2(4) 4_575 4_675 ?
O9 Cs3 O8 48.9(3) 4_675 4_675 ?
O22 Cs3 O8 79.7(3) 4_675 4_675 ?
O26 Cs3 O8 146.4(3) . 4_675 ?
O28 Cs3 O8 97.2(3) . 4_675 ?
O13 Cs3 O8 161.5(3) . 4_675 ?
O17 Cs3 Mo1 137.5(3) 4_575 4_675 ?
O9 Cs3 Mo1 27.5(2) 4_675 4_675 ?
O22 Cs3 Mo1 24.5(2) 4_675 4_675 ?
O26 Cs3 Mo1 123.6(2) . 4_675 ?
O28 Cs3 Mo1 106.8(2) . 4_675 ?
O13 Cs3 Mo1 95.9(2) . 4_675 ?
O8 Cs3 Mo1 66.7(2) 4_675 4_675 ?
O17 Cs3 V2 130.6(3) 4_575 4_675 ?
O9 Cs3 V2 26.6(2) 4_675 4_675 ?
O22 Cs3 V2 63.1(2) 4_675 4_675 ?
O26 Cs3 V2 142.9(2) . 4_675 ?
O28 Cs3 V2 95.3(2) . 4_675 ?
O13 Cs3 V2 141.5(2) . 4_675 ?
O8 Cs3 V2 22.5(2) 4_675 4_675 ?
Mo1 Cs3 V2 45.68(5) 4_675 4_675 ?
O17 Cs3 Na1 78.2(4) 4_575 . ?
O9 Cs3 Na1 75.3(3) 4_675 . ?
O22 Cs3 Na1 56.1(3) 4_675 . ?
O26 Cs3 Na1 157.4(3) . . ?
O28 Cs3 Na1 151.3(3) . . ?
O13 Cs3 Na1 114.2(3) . . ?
O8 Cs3 Na1 54.3(3) 4_675 . ?
Mo1 Cs3 Na1 66.70(13) 4_675 . ?
V2 Cs3 Na1 59.48(13) 4_675 . ?
O17 Cs3 Mo4 18.7(3) 4_575 4_575 ?
O9 Cs3 Mo4 136.4(2) 4_675 4_575 ?
O22 Cs3 Mo4 110.7(2) 4_675 4_575 ?
O26 Cs3 Mo4 99.5(2) . 4_575 ?
O28 Cs3 Mo4 121.7(3) . 4_575 ?
O13 Cs3 Mo4 94.1(3) . 4_575 ?
O8 Cs3 Mo4 92.6(2) 4_675 4_575 ?
Mo1 Cs3 Mo4 129.51(7) 4_675 4_575 ?
V2 Cs3 Mo4 112.10(7) 4_675 4_575 ?
Na1 Cs3 Mo4 64.07(13) . 4_575 ?
O17 Cs3 Na3 55.4(3) 4_575 4_575 ?
O9 Cs3 Na3 124.8(3) 4_675 4_575 ?
O22 Cs3 Na3 152.8(4) 4_675 4_575 ?
O26 Cs3 Na3 82.1(4) . 4_575 ?
O28 Cs3 Na3 74.3(3) . 4_575 ?
O13 Cs3 Na3 115.6(4) . 4_575 ?
O8 Cs3 Na3 81.7(4) 4_675 4_575 ?
Mo1 Cs3 Na3 148.4(3) 4_675 4_575 ?
V2 Cs3 Na3 102.8(3) 4_675 4_575 ?
Na1 Cs3 Na3 96.8(3) . 4_575 ?
Mo4 Cs3 Na3 50.50(18) 4_575 4_575 ?
O78 Cs4 O23 120.7(8) . 4_675 ?
O78 Cs4 O13 122.6(8) . . ?
O23 Cs4 O13 107.5(4) 4_675 . ?
O78 Cs4 O29 89.2(8) . 2_556 ?
O23 Cs4 O29 115.7(4) 4_675 2_556 ?
O13 Cs4 O29 96.9(3) . 2_556 ?
O78 Cs4 O31 92.1(8) . 2_556 ?
O23 Cs4 O31 66.7(3) 4_675 2_556 ?
O13 Cs4 O31 137.2(4) . 2_556 ?
O29 Cs4 O31 55.9(3) 2_556 2_556 ?
O78 Cs4 O30 52.1(8) . 2_556 ?
O23 Cs4 O30 106.9(3) 4_675 2_556 ?
O13 Cs4 O30 138.9(3) . 2_556 ?
O29 Cs4 O30 47.2(3) 2_556 2_556 ?
O31 Cs4 O30 45.8(3) 2_556 2_556 ?
O78 Cs4 O74 133.2(9) . 2_556 ?
O23 Cs4 O74 72.1(5) 4_675 2_556 ?
O13 Cs4 O74 88.4(5) . 2_556 ?
O29 Cs4 O74 49.8(5) 2_556 2_556 ?
O31 Cs4 O74 48.9(5) 2_556 2_556 ?
O30 Cs4 O74 81.3(5) 2_556 2_556 ?
O78 Cs4 O14 81.1(8) . . ?
O23 Cs4 O14 119.0(3) 4_675 . ?
O13 Cs4 O14 47.4(3) . . ?
O29 Cs4 O14 121.1(3) 2_556 . ?
O31 Cs4 O14 172.7(3) 2_556 . ?
O30 Cs4 O14 127.0(3) 2_556 . ?
O74 Cs4 O14 135.6(5) 2_556 . ?
O78 Cs4 O16 62.9(8) . . ?
O23 Cs4 O16 92.4(3) 4_675 . ?
O13 Cs4 O16 87.2(3) . . ?
O29 Cs4 O16 148.4(4) 2_556 . ?
O31 Cs4 O16 133.9(3) 2_556 . ?
O30 Cs4 O16 113.2(3) 2_556 . ?
O74 Cs4 O16 161.7(5) 2_556 . ?
O14 Cs4 O16 44.4(3) . . ?
O78 Cs4 Mo5 66.7(8) . 2_556 ?
O23 Cs4 Mo5 123.1(3) 4_675 2_556 ?
O13 Cs4 Mo5 111.6(2) . 2_556 ?
O29 Cs4 Mo5 22.8(2) 2_556 2_556 ?
O31 Cs4 Mo5 56.6(2) 2_556 2_556 ?
O30 Cs4 Mo5 28.0(2) 2_556 2_556 ?
O74 Cs4 Mo5 69.5(4) 2_556 2_556 ?
O14 Cs4 Mo5 117.8(2) . 2_556 ?
O16 Cs4 Mo5 128.5(3) . 2_556 ?
O78 Cs4 Mo1 140.5(7) . 4_675 ?
O23 Cs4 Mo1 20.1(2) 4_675 4_675 ?
O13 Cs4 Mo1 91.8(3) . 4_675 ?
O29 Cs4 Mo1 106.5(3) 2_556 4_675 ?
O31 Cs4 Mo1 69.6(2) 2_556 4_675 ?
O30 Cs4 Mo1 114.9(2) 2_556 4_675 ?
O74 Cs4 Mo1 57.9(5) 2_556 4_675 ?
O14 Cs4 Mo1 117.3(2) . 4_675 ?
O16 Cs4 Mo1 104.6(2) . 4_675 ?
Mo5 Cs4 Mo1 121.38(10) 2_556 4_675 ?
O78 Cs4 Mo6 70.2(8) . 2_556 ?
O23 Cs4 Mo6 81.3(2) 4_675 2_556 ?
O13 Cs4 Mo6 151.1(3) . 2_556 ?
O29 Cs4 Mo6 55.4(2) 2_556 2_556 ?
O31 Cs4 Mo6 22.0(2) 2_556 2_556 ?
O30 Cs4 Mo6 26.1(2) 2_556 2_556 ?
O74 Cs4 Mo6 67.7(4) 2_556 2_556 ?
O14 Cs4 Mo6 150.9(2) . 2_556 ?
O16 Cs4 Mo6 120.5(2) . 2_556 ?
Mo5 Cs4 Mo6 45.94(4) 2_556 2_556 ?
Mo1 Cs4 Mo6 88.99(7) 4_675 2_556 ?
Na4 Na1 Cs3 131.8(4) 3_576 . ?
Na4 Na1 Cs2 55.2(2) 3_576 3_576 ?
Cs3 Na1 Cs2 143.5(3) . 3_576 ?
O18 P1 O20 110.7(8) . . ?
O18 P1 O19 110.0(7) . . ?
O20 P1 O19 110.2(7) . . ?
O18 P1 O25 108.4(7) . . ?
O20 P1 O25 109.5(7) . . ?
O19 P1 O25 107.9(7) . . ?
O18 P1 Cs2 47.0(5) . 3_577 ?
O20 P1 Cs2 67.4(5) . 3_577 ?
O19 P1 Cs2 109.3(5) . 3_577 ?
O25 P1 Cs2 141.0(5) . 3_577 ?
V1 O2 Ru1 151.7(8) . . ?
V1 O2 Cs2 107.4(5) . . ?
Ru1 O2 Cs2 100.4(5) . . ?
V2 O3 Ru1 150.8(7) 3_577 . ?
V3 O4 Ru1 121.4(6) . . ?
V3 O4 Cs2 131.4(6) . . ?
Ru1 O4 Cs2 104.5(4) . . ?
V3 O5 Cs1 129.7(6) . 4_575 ?
V3 O6 V1 129.0(7) . 3_577 ?
V3 O6 Mo3 117.9(6) . . ?
V1 O6 Mo3 100.0(5) 3_577 . ?
V3 O7 V2 129.5(6) . . ?
V3 O7 Mo2 118.9(6) . . ?
V2 O7 Mo2 99.9(5) . . ?
V2 O8 Cs3 104.6(6) . 4_576 ?
V2 O9 Mo1 112.5(6) . . ?
V2 O9 Cs3 103.9(5) . 4_576 ?
Mo1 O9 Cs3 102.2(5) . 4_576 ?
Mo2 O10 V2 110.7(6) . . ?
Mo2 O10 Mo1 141.3(6) . . ?
V2 O10 Mo1 95.9(5) . . ?
Mo2 O11 Cs2 107.0(5) . 2_446 ?
Mo2 O11 Cs1 125.1(5) . 4_575 ?
Cs2 O11 Cs1 108.3(4) 2_446 4_575 ?
Mo3 O12 Mo2 119.2(6) . . ?
Mo3 O13 Cs4 114.0(6) . . ?
Mo3 O13 Cs3 102.7(5) . . ?
Cs4 O13 Cs3 95.5(4) . . ?
Mo3 O14 V1 111.2(6) . 3_577 ?
Mo3 O14 Mo4 140.4(7) . . ?
V1 O14 Mo4 96.3(6) 3_577 . ?
Mo3 O14 Cs4 95.4(5) . . ?
V1 O14 Cs4 100.1(5) 3_577 . ?
Mo4 O14 Cs4 107.5(4) . . ?
V1 O15 Mo4 111.8(7) 3_577 . ?
V1 O15 Na3 127.1(8) 3_577 . ?
Mo4 O15 Na3 116.6(7) . . ?
V1 O15 Cs2 99.1(5) 3_577 3_577 ?
Mo4 O15 Cs2 105.5(5) . 3_577 ?
Na3 O15 Cs2 87.7(7) . 3_577 ?
Mo4 O16 Cs4 117.6(7) . . ?
Mo4 O17 Cs3 125.0(8) . 4_676 ?
P1 O18 Mo4 137.4(9) . . ?
P1 O18 Cs2 112.0(7) . 3_577 ?
Mo4 O18 Cs2 107.7(5) . 3_577 ?
P1 O19 Mo2 127.2(6) . . ?
P1 O19 Mo3 125.7(6) . . ?
Mo2 O19 Mo3 92.4(4) . . ?
P1 O20 Mo1 134.5(7) . . ?
P1 O20 Cs1 100.3(5) . . ?
Mo1 O20 Cs1 88.0(4) . . ?
P1 O20 Cs2 89.7(5) . 3_577 ?
Mo1 O20 Cs2 133.7(5) . 3_577 ?
Cs1 O20 Cs2 98.5(3) . 3_577 ?
Mo2 O21 Mo6 143.0(7) . . ?
Mo2 O21 Cs2 98.6(5) . 2_446 ?
Mo6 O21 Cs2 111.0(4) . 2_446 ?
Mo1 O22 Cs3 105.5(5) . 4_576 ?
Mo1 O23 Cs1 113.0(6) . . ?
Mo1 O23 Cs4 121.0(6) . 4_576 ?
Cs1 O23 Cs4 110.3(4) . 4_576 ?
Mo6 O24 Mo1 162.5(7) . . ?
Mo6 O24 Cs1 90.3(4) . . ?
Mo1 O24 Cs1 85.3(4) . . ?
P1 O25 Mo5 127.9(7) . . ?
P1 O25 Mo6 128.2(7) . . ?
Mo5 O25 Mo6 94.9(5) . . ?
P1 O25 Cs1 93.1(6) . . ?
Mo5 O25 Cs1 120.4(4) . . ?
Mo6 O25 Cs1 86.6(4) . . ?
Mo3 O26 Mo5 143.9(7) . . ?
Mo3 O26 Cs3 105.1(5) . . ?
Mo5 O26 Cs3 103.6(4) . . ?
Mo5 O27 Mo4 160.3(8) . . ?
Mo5 O28 Cs3 121.4(6) . . ?
Mo5 O29 Cs4 107.1(6) . 2_546 ?
Mo6 O30 Mo5 117.2(7) . . ?
Mo6 O30 Cs4 99.8(5) . 2_546 ?
Mo5 O30 Cs4 93.3(4) . 2_546 ?
Mo6 O31 Cs1 108.3(6) . . ?
Mo6 O31 Cs1 96.5(5) . 3_567 ?
Cs1 O31 Cs1 118.5(4) . 3_567 ?
Mo6 O31 Cs4 106.9(6) . 2_546 ?
Cs1 O31 Cs4 129.7(4) . 2_546 ?
Cs1 O31 Cs4 91.6(3) 3_567 2_546 ?
Mo6 O32 Cs1 107.8(6) . 3_567 ?
Mo6 O32 Cs2 119.3(5) . 2_446 ?
Cs1 O32 Cs2 129.4(4) 3_567 2_446 ?
Na3 O34 Cs2 93.2(9) 3_577 . ?
Na1 Na4 Cs2 76.4(3) 3_576 . ?
Na1 Na4 Cs3 104.7(3) 3_576 2_556 ?
Cs2 Na4 Cs3 126.4(4) . 2_556 ?
O34 Na3 O15 93.1(9) 3_577 . ?
O34 Na3 O78 85.3(12) 3_577 3_677 ?
O15 Na3 O78 173.1(14) . 3_677 ?
O34 Na3 Mo4 115.0(9) 3_577 . ?
O15 Na3 Mo4 27.4(3) . . ?
O78 Na3 Mo4 149.4(11) 3_677 . ?
O34 Na3 Na3 125.6(11) 3_577 3_677 ?
O15 Na3 Na3 102.3(9) . 3_677 ?
O78 Na3 Na3 84.0(10) 3_677 3_677 ?
Mo4 Na3 Na3 100.1(7) . 3_677 ?
O34 Na3 Cs2 51.9(8) 3_577 3_577 ?
O15 Na3 Cs2 55.5(5) . 3_577 ?
O78 Na3 Cs2 119.0(11) 3_677 3_577 ?
Mo4 Na3 Cs2 66.6(2) . 3_577 ?
Na3 Na3 Cs2 154.3(8) 3_677 3_577 ?
O34 Na3 Cs3 140.1(11) 3_577 4_676 ?
O15 Na3 Cs3 91.8(5) . 4_676 ?
O78 Na3 Cs3 85.2(10) 3_677 4_676 ?
Mo4 Na3 Cs3 64.4(2) . 4_676 ?
Na3 Na3 Cs3 91.8(5) 3_677 4_676 ?
Cs2 Na3 Cs3 101.0(4) 3_577 4_676 ?
O34 Na3 Cs4 75.0(8) 3_577 3_677 ?
O15 Na3 Cs4 166.5(8) . 3_677 ?
O78 Na3 Cs4 10.3(9) 3_677 3_677 ?
Mo4 Na3 Cs4 155.7(5) . 3_677 ?
Na3 Na3 Cs4 90.0(4) 3_677 3_677 ?
Cs2 Na3 Cs4 111.2(5) 3_577 3_677 ?
Cs3 Na3 Cs4 93.4(3) 4_676 3_677 ?
Cs1 O74 Cs4 125.2(9) . 2_546 ?
Na3 O78 Cs4 159.9(16) 3_677 . ?

_refine_diff_density_max         5.614
_refine_diff_density_min         -4.574
_refine_diff_density_rms         0.364



####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_pna2
_database_code_depnum_ccdc_archive 'CCDC 2041201'
loop_
_audit_author_name
_audit_author_address
'ai-quan jia'
;anhui university of technology
China
;
_audit_update_record             
;
2020-10-29 deposited with the CCDC.	2020-12-02 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2016/6
_shelx_SHELXL_version_number     2016/6
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C6 H18 Cs3 Mo6 Na3 O40 P Ru S3 V3'
_chemical_formula_weight         2154.58

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.1246 0.1234 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ru Ru -1.2594 0.8363 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      orthorhombic
_space_group_IT_number           33
_space_group_name_H-M_alt        'P n a 21'
_space_group_name_Hall           'P 2c -2n'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z+1/2'
'x+1/2, -y+1/2, z'
'-x+1/2, y+1/2, z+1/2'

_cell_length_a                   20.2810(16)
_cell_length_b                   19.8627(15)
_cell_length_c                   13.2758(10)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     5348.0(7)
_cell_formula_units_Z            4
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    9917
_cell_measurement_theta_min      2.25
_cell_measurement_theta_max      30.38

_exptl_crystal_description       block
_exptl_crystal_colour            brown
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    2.676
_exptl_crystal_F_000             4000
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          0.280
_exptl_crystal_size_mid          0.220
_exptl_crystal_size_min          0.160
_exptl_absorpt_coefficient_mu    4.406
_shelx_estimated_absorpt_T_min   0.372
_shelx_estimated_absorpt_T_max   0.539
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.325
_exptl_absorpt_correction_T_max  0.494
_exptl_absorpt_process_details   sadabs
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'Bruker P4'
_diffrn_measurement_method       'ω scans'
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            28719
_diffrn_reflns_av_unetI/netI     0.0271
_diffrn_reflns_av_R_equivalents  0.0216
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_k_max       21
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_theta_min         1.845
_diffrn_reflns_theta_max         25.000
_diffrn_reflns_theta_full        25.000
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measured_fraction_theta_full 0.993
_diffrn_reflns_Laue_measured_fraction_max 0.993
_diffrn_reflns_Laue_measured_fraction_full 0.993
_diffrn_reflns_point_group_measured_fraction_max 0.994
_diffrn_reflns_point_group_measured_fraction_full 0.994
_reflns_number_total             9354
_reflns_number_gt                9111
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.911
_reflns_Friedel_fraction_max     0.995
_reflns_Friedel_fraction_full    0.995

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       'Bruker XSCANS'
_computing_cell_refinement       'Bruker XSCANS'
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0100P)²+200.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   geom
_refine_ls_hydrogen_treatment    constr
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.98(5)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         9354
_refine_ls_number_parameters     596
_refine_ls_number_restraints     1635
_refine_ls_R_factor_all          0.0539
_refine_ls_R_factor_gt           0.0526
_refine_ls_wR_factor_ref         0.1359
_refine_ls_wR_factor_gt          0.1354
_refine_ls_goodness_of_fit_ref   1.154
_refine_ls_restrained_S_all      1.221
_refine_ls_shift/su_max          0.013
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Ru1 Ru 0.36670(7) 1.02570(7) 0.32582(11) 0.0121(3) Uani 1 1 d . U . . .
Mo1 Mo 0.31254(10) 0.78137(9) 0.03933(14) 0.0247(4) Uani 1 1 d . U . . .
Mo2 Mo 0.46917(8) 0.76655(8) 0.20272(12) 0.0149(3) Uani 1 1 d . U . . .
Mo3 Mo 0.45003(8) 0.76045(8) 0.45165(12) 0.0152(3) Uani 1 1 d . U . . .
Mo4 Mo 0.26852(9) 0.76956(9) 0.54923(14) 0.0216(4) Uani 1 1 d . U . . .
Mo5 Mo 0.34561(10) 0.61712(9) 0.17266(14) 0.0232(4) Uani 1 1 d . U . . .
Mo6 Mo 0.32451(10) 0.61096(9) 0.41920(14) 0.0230(4) Uani 1 1 d . U . . .
V1 V 0.39300(17) 0.90056(16) 0.1323(2) 0.0139(6) Uani 1 1 d . U . . .
V2 V 0.48885(15) 0.91532(15) 0.3408(2) 0.0121(6) Uani 1 1 d . U . . .
V3 V 0.36553(17) 0.89063(16) 0.5143(2) 0.0152(7) Uani 1 1 d . U . . .
Cs1 Cs 0.35734(9) 0.95223(8) -0.15470(11) 0.0398(4) Uani 1 1 d . U . . .
Cs2 Cs 0.40074(14) 0.64101(17) 0.6858(2) 0.0873(8) Uani 1 1 d . U . . .
Cs3 Cs 0.1572(2) 0.6909(3) 0.2814(6) 0.180(2) Uani 1 1 d . U . . .
Na1 Na 0.0972(5) 0.7796(5) 0.6588(7) 0.032(2) Uani 1 1 d . U . . .
Na2 Na 0.2238(5) 0.7188(4) 0.8280(8) 0.038(2) Uani 1 1 d . U . . .
S1 S 0.3836(2) 1.1019(2) 0.2018(4) 0.0172(10) Uani 1 1 d . U . . .
S2 S 0.2576(2) 1.0439(2) 0.3243(4) 0.0188(10) Uani 1 1 d . U . . .
S3 S 0.3875(3) 1.1045(2) 0.4446(4) 0.0178(10) Uani 1 1 d . U . . .
P1 P 0.3106(3) 0.7645(2) 0.2987(4) 0.0152(10) Uani 1 1 d . U . . .
O1 O 0.3723(8) 1.1738(7) 0.2263(11) 0.026(3) Uani 1 1 d . U . . .
O2 O 0.2305(8) 1.1099(8) 0.2868(14) 0.035(3) Uani 1 1 d . U . . .
O3 O 0.3369(8) 1.1546(7) 0.4515(12) 0.034(3) Uani 1 1 d D U . . .
O4 O 0.3579(7) 0.9504(7) 0.2196(10) 0.0183(19) Uani 1 1 d . U . . .
O5 O 0.4653(6) 0.9973(6) 0.3363(11) 0.016(2) Uani 1 1 d . U . . .
O6 O 0.3514(7) 0.9547(7) 0.4347(10) 0.0192(19) Uani 1 1 d . U . . .
O7 O 0.4318(7) 0.9493(7) 0.0545(11) 0.021(2) Uani 1 1 d . U . . .
O8 O 0.5690(7) 0.9143(7) 0.3548(11) 0.021(2) Uani 1 1 d . U . . .
O9 O 0.3909(7) 0.9230(7) 0.6182(10) 0.020(2) Uani 1 1 d . U . . .
O10 O 0.3199(7) 0.8770(7) 0.0511(11) 0.022(2) Uani 1 1 d . U . . .
O11 O 0.4679(7) 0.8766(7) 0.2214(10) 0.0175(18) Uani 1 1 d . U . . .
O12 O 0.4500(7) 0.8697(7) 0.4444(10) 0.0180(18) Uani 1 1 d . U . . .
O13 O 0.2778(7) 0.8657(7) 0.5476(11) 0.024(2) Uani 1 1 d . U . . .
O14 O 0.2818(8) 0.7526(8) 0.6745(12) 0.034(2) Uani 1 1 d . U . . .
O15 O 0.2297(8) 0.7797(7) 0.0149(13) 0.034(3) Uani 1 1 d . U . . .
O16 O 0.3479(9) 0.7682(8) -0.0785(12) 0.033(3) Uani 1 1 d . U . . .
O17 O 0.4090(7) 0.8021(7) 0.1074(10) 0.0195(18) Uani 1 1 d . U . . .
O18 O 0.2835(8) 0.7918(8) 0.2025(12) 0.0267(19) Uani 1 1 d . U . . .
O19 O 0.3850(7) 0.7849(7) 0.3152(10) 0.0204(17) Uani 1 1 d . U . . .
O20 O 0.2691(8) 0.7895(8) 0.3839(11) 0.0274(19) Uani 1 1 d . U . . .
O21 O 0.3760(7) 0.7910(7) 0.5270(11) 0.0222(18) Uani 1 1 d . U . . .
O22 O 0.1853(8) 0.7635(8) 0.5414(14) 0.036(2) Uani 1 1 d . U . . .
O24 O 0.5076(7) 0.7686(6) 0.3370(11) 0.0202(19) Uani 1 1 d . U . . .
O25 O 0.5420(7) 0.7660(7) 0.1361(11) 0.021(2) Uani 1 1 d . U . . .
O26 O 0.3296(8) 0.6911(7) 0.0863(11) 0.026(2) Uani 1 1 d . U . . .
O27 O 0.4428(7) 0.6853(7) 0.1976(11) 0.022(2) Uani 1 1 d . U . . .
O28 O 0.3059(8) 0.6861(7) 0.2930(11) 0.0260(18) Uani 1 1 d . U . . .
O29 O 0.4224(8) 0.6780(7) 0.4396(11) 0.024(2) Uani 1 1 d . U . . .
O30 O 0.2951(8) 0.6815(8) 0.5022(11) 0.0272(19) Uani 1 1 d . U . . .
O31 O 0.3951(9) 0.5684(8) 0.0997(12) 0.034(3) Uani 1 1 d . U . . .
O32 O 0.2686(9) 0.5790(9) 0.1651(13) 0.038(2) Uani 1 1 d . U . . .
O33 O 0.3742(8) 0.5814(7) 0.3022(11) 0.027(2) Uani 1 1 d . U . . .
O34 O 0.2503(9) 0.5731(8) 0.3940(13) 0.0360(18) Uani 1 1 d . U . . .
O35 O 0.3620(9) 0.5567(8) 0.5044(13) 0.0360(18) Uani 1 1 d . U . . .
O38 O 0.1687(10) 0.8209(9) 0.7982(15) 0.050(3) Uani 1 1 d . U . . .
O41 O 0.1323(9) 0.7819(12) 0.3686(16) 0.058(4) Uani 1 1 d . U . . .
O42 O 0.1563(10) 0.8363(12) 0.2080(16) 0.057(4) Uani 1 1 d . U . . .
O43 O 0.1592(11) 0.7332(12) 0.1364(15) 0.068(4) Uani 1 1 d . U . . .
C1 C 0.3349(12) 1.0864(12) 0.0907(17) 0.030(4) Uani 1 1 d . U . . .
H1A H 0.289400 1.095738 0.104993 0.045 Uiso 1 1 calc R U . . .
H1B H 0.339577 1.040194 0.070900 0.045 Uiso 1 1 calc R U . . .
H1C H 0.349757 1.115111 0.037155 0.045 Uiso 1 1 calc R U . . .
C2 C 0.4657(11) 1.0948(10) 0.1513(15) 0.022(4) Uani 1 1 d . U . . .
H2A H 0.467182 1.115215 0.085752 0.033 Uiso 1 1 calc R U . . .
H2B H 0.477516 1.048137 0.145944 0.033 Uiso 1 1 calc R U . . .
H2C H 0.496190 1.117300 0.195162 0.033 Uiso 1 1 calc R U . . .
C3 C 0.2197(12) 0.9796(14) 0.255(2) 0.040(4) Uani 1 1 d . U . . .
H3A H 0.173146 0.979641 0.268368 0.059 Uiso 1 1 calc R U . . .
H3B H 0.238061 0.936967 0.274116 0.059 Uiso 1 1 calc R U . . .
H3C H 0.226993 0.986999 0.184368 0.059 Uiso 1 1 calc R U . . .
C4 C 0.2240(13) 1.0289(14) 0.440(2) 0.042(4) Uani 1 1 d . U . . .
H4A H 0.179346 1.044946 0.441453 0.063 Uiso 1 1 calc R U . . .
H4B H 0.249264 1.051880 0.490727 0.063 Uiso 1 1 calc R U . . .
H4C H 0.224475 0.981379 0.453525 0.063 Uiso 1 1 calc R U . . .
C5 C 0.4642(11) 1.1441(11) 0.4237(17) 0.027(4) Uani 1 1 d . U . . .
H5A H 0.459640 1.177031 0.371281 0.040 Uiso 1 1 calc R U . . .
H5B H 0.496200 1.111023 0.404018 0.040 Uiso 1 1 calc R U . . .
H5C H 0.478439 1.165803 0.484582 0.040 Uiso 1 1 calc R U . . .
C6 C 0.4031(12) 1.0666(12) 0.5641(16) 0.028(4) Uani 1 1 d . U . . .
H6A H 0.418024 1.100391 0.610541 0.042 Uiso 1 1 calc R U . . .
H6B H 0.436399 1.032623 0.556916 0.042 Uiso 1 1 calc R U . . .
H6C H 0.363282 1.046550 0.589059 0.042 Uiso 1 1 calc R U . . .
O50 O 0.5100(7) 0.7552(7) 0.5404(12) 0.026(2) Uani 1 1 d . U . . .
Na3 Na 0.2273(11) 0.9329(9) -0.293(2) 0.130(9) Uani 1 1 d . . . . .
O51 O 0.0806(15) 0.8939(12) 0.621(2) 0.082(6) Uani 1 1 d . U . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Ru1 O6 2.044(14) . ?
Ru1 O4 2.064(14) . ?
Ru1 O5 2.083(13) . ?
Ru1 S2 2.243(5) . ?
Ru1 S3 2.261(5) . ?
Ru1 S1 2.263(5) . ?
Mo1 O15 1.711(16) . ?
Mo1 O16 1.741(17) . ?
Mo1 O10 1.912(14) . ?
Mo1 O26 1.929(15) . ?
Mo1 O17 2.194(15) . ?
Mo1 O18 2.255(16) . ?
Mo1 V1 3.129(4) . ?
Mo1 Na2 3.558(10) 1_554 ?
Mo2 O27 1.701(14) . ?
Mo2 O25 1.721(14) . ?
Mo2 O17 1.894(14) . ?
Mo2 O24 1.945(15) . ?
Mo2 O11 2.200(14) . ?
Mo2 O19 2.298(14) . ?
Mo2 Cs3 4.044(5) 3_565 ?
Mo3 O50 1.696(14) . ?
Mo3 O29 1.738(14) . ?
Mo3 O21 1.904(14) . ?
Mo3 O24 1.925(15) . ?
Mo3 O12 2.172(13) . ?
Mo3 O19 2.293(14) . ?
Mo4 O22 1.695(17) . ?
Mo4 O14 1.717(16) . ?
Mo4 O13 1.919(14) . ?
Mo4 O30 1.933(16) . ?
Mo4 O20 2.230(15) . ?
Mo4 O21 2.240(14) . ?
Mo4 V3 3.142(4) . ?
Mo4 Cs3 4.492(7) . ?
Mo5 O31 1.697(17) . ?
Mo5 O32 1.739(16) . ?
Mo5 O26 1.892(15) . ?
Mo5 O33 1.948(15) . ?
Mo5 O28 2.253(15) . ?
Mo5 O27 2.414(14) . ?
Mo5 Cs3 4.339(6) . ?
Mo6 O34 1.716(17) . ?
Mo6 O35 1.738(18) . ?
Mo6 O30 1.880(16) . ?
Mo6 O33 1.943(15) . ?
Mo6 O28 2.275(15) . ?
Mo6 O29 2.407(15) . ?
Mo6 Cs3 4.168(6) . ?
V1 O7 1.620(14) . ?
V1 O4 1.682(14) . ?
V1 O10 1.891(14) . ?
V1 O11 1.984(14) . ?
V1 O17 2.011(14) . ?
V2 O8 1.636(14) . ?
V2 O5 1.698(12) . ?
V2 O11 1.812(13) . ?
V2 O12 1.825(14) . ?
V2 Cs1 4.081(3) 2_675 ?
V2 Cs3 4.090(6) 3_565 ?
V3 O9 1.607(14) . ?
V3 O6 1.678(14) . ?
V3 O13 1.899(15) . ?
V3 O12 1.992(14) . ?
V3 O21 1.997(15) . ?
Cs1 O8 3.045(14) 2_674 ?
Cs1 O9 3.145(14) 1_554 ?
Cs1 O7 3.162(14) . ?
Cs1 O10 3.205(14) . ?
Cs1 O34 3.308(16) 4_554 ?
Cs1 O5 3.736(13) 2_674 ?
Cs1 O16 3.797(17) . ?
Cs1 Cs3 4.824(6) 4_554 ?
Cs2 O35 3.037(17) . ?
Cs2 O2 3.044(17) 4_545 ?
Cs2 O14 3.280(18) . ?
Cs2 O30 3.344(17) . ?
Cs2 O29 3.379(15) . ?
Cs2 O21 3.684(15) . ?
Cs2 O50 3.712(16) . ?
Cs2 S2 4.172(6) 4_545 ?
Cs2 Na1 4.300(10) 3_565 ?
Cs3 O41 2.21(3) . ?
Cs3 O43 2.10(3) . ?
Cs3 O8 2.918(15) 3_465 ?
Cs3 O28 3.021(17) . ?
Cs3 O42 3.05(2) . ?
Cs3 O25 3.149(16) 3_465 ?
Cs3 O24 3.226(15) 3_465 ?
Cs3 O20 3.293(17) . ?
Cs3 O34 3.357(19) . ?
Cs3 O18 3.417(17) . ?
Cs3 P1 3.446(7) . ?
Cs3 O32 3.52(2) . ?
Na1 O51 2.35(2) . ?
Na1 O1 2.367(18) 4_545 ?
Na1 O22 2.392(19) . ?
Na1 O50 2.465(17) 3_465 ?
Na1 O38 2.49(2) . ?
Na1 Na3 4.08(2) 1_556 ?
Na2 O38 2.35(2) . ?
Na2 O2 2.42(2) 4_545 ?
Na2 O14 2.448(19) . ?
Na2 O3 2.414(18) 4_545 ?
Na2 O1 2.533(18) 4_545 ?
Na2 O15 2.762(19) 1_556 ?
Na2 O16 2.97(2) 1_556 ?
S1 O1 1.483(15) . ?
S1 C2 1.80(2) . ?
S1 C1 1.80(2) . ?
S2 O2 1.506(16) . ?
S2 C4 1.71(2) . ?
S2 C3 1.75(2) . ?
S3 O3 1.433(14) . ?
S3 C5 1.77(2) . ?
S3 C6 1.78(2) . ?
P1 O18 1.493(16) . ?
P1 O20 1.496(15) . ?
P1 O28 1.563(15) . ?
P1 O19 1.576(15) . ?
O13 Na3 2.70(3) 1_556 ?
O32 Na3 2.96(3) 4_545 ?
O38 Na3 2.80(3) 1_556 ?
C1 H1A 0.9600 . ?
C1 H1B 0.9600 . ?
C1 H1C 0.9600 . ?
C2 H2A 0.9600 . ?
C2 H2B 0.9600 . ?
C2 H2C 0.9600 . ?
C3 H3A 0.9600 . ?
C3 H3B 0.9600 . ?
C3 H3C 0.9600 . ?
C4 H4A 0.9600 . ?
C4 H4B 0.9600 . ?
C4 H4C 0.9600 . ?
C5 H5A 0.9600 . ?
C5 H5B 0.9600 . ?
C5 H5C 0.9600 . ?
C6 H6A 0.9600 . ?
C6 H6B 0.9600 . ?
C6 H6C 0.9600 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O6 Ru1 O4 88.3(5) . . ?
O6 Ru1 O5 84.9(5) . . ?
O4 Ru1 O5 86.1(5) . . ?
O6 Ru1 S2 88.2(4) . . ?
O4 Ru1 S2 91.5(4) . . ?
O5 Ru1 S2 172.7(4) . . ?
O6 Ru1 S3 90.7(4) . . ?
O4 Ru1 S3 173.9(4) . . ?
O5 Ru1 S3 87.8(4) . . ?
S2 Ru1 S3 94.54(19) . . ?
O6 Ru1 S1 178.3(4) . . ?
O4 Ru1 S1 90.0(4) . . ?
O5 Ru1 S1 94.8(4) . . ?
S2 Ru1 S1 92.01(19) . . ?
S3 Ru1 S1 90.98(17) . . ?
O15 Mo1 O16 103.4(8) . . ?
O15 Mo1 O10 96.4(7) . . ?
O16 Mo1 O10 100.9(7) . . ?
O15 Mo1 O26 102.7(7) . . ?
O16 Mo1 O26 94.5(7) . . ?
O10 Mo1 O26 152.0(6) . . ?
O15 Mo1 O17 163.2(7) . . ?
O16 Mo1 O17 91.8(7) . . ?
O10 Mo1 O17 73.2(6) . . ?
O26 Mo1 O17 83.2(6) . . ?
O15 Mo1 O18 85.9(7) . . ?
O16 Mo1 O18 170.1(7) . . ?
O10 Mo1 O18 81.4(6) . . ?
O26 Mo1 O18 79.7(6) . . ?
O17 Mo1 O18 79.6(5) . . ?
O15 Mo1 V1 127.0(5) . . ?
O16 Mo1 V1 104.6(6) . . ?
O10 Mo1 V1 34.4(4) . . ?
O26 Mo1 V1 118.8(5) . . ?
O17 Mo1 V1 39.7(4) . . ?
O18 Mo1 V1 71.8(4) . . ?
O15 Mo1 Na2 49.2(6) . 1_554 ?
O16 Mo1 Na2 56.5(6) . 1_554 ?
O10 Mo1 Na2 116.8(4) . 1_554 ?
O26 Mo1 Na2 91.2(5) . 1_554 ?
O17 Mo1 Na2 147.3(4) . 1_554 ?
O18 Mo1 Na2 131.1(4) . 1_554 ?
V1 Mo1 Na2 147.06(17) . 1_554 ?
O27 Mo2 O25 104.1(7) . . ?
O27 Mo2 O17 97.1(7) . . ?
O25 Mo2 O17 102.2(7) . . ?
O27 Mo2 O24 100.5(6) . . ?
O25 Mo2 O24 97.3(7) . . ?
O17 Mo2 O24 149.6(6) . . ?
O27 Mo2 O11 160.6(6) . . ?
O25 Mo2 O11 94.2(6) . . ?
O17 Mo2 O11 72.4(5) . . ?
O24 Mo2 O11 83.1(5) . . ?
O27 Mo2 O19 86.7(6) . . ?
O25 Mo2 O19 166.5(6) . . ?
O17 Mo2 O19 84.1(6) . . ?
O24 Mo2 O19 72.5(5) . . ?
O11 Mo2 O19 76.2(5) . . ?
O27 Mo2 Cs3 120.4(5) . 3_565 ?
O25 Mo2 Cs3 47.5(5) . 3_565 ?
O17 Mo2 Cs3 134.6(5) . 3_565 ?
O24 Mo2 Cs3 51.8(4) . 3_565 ?
O11 Mo2 Cs3 76.9(4) . 3_565 ?
O19 Mo2 Cs3 120.0(4) . 3_565 ?
O50 Mo3 O29 103.7(7) . . ?
O50 Mo3 O21 102.7(7) . . ?
O29 Mo3 O21 95.4(7) . . ?
O50 Mo3 O24 96.9(7) . . ?
O29 Mo3 O24 101.6(6) . . ?
O21 Mo3 O24 150.1(6) . . ?
O50 Mo3 O12 95.3(6) . . ?
O29 Mo3 O12 159.6(6) . . ?
O21 Mo3 O12 72.8(6) . . ?
O24 Mo3 O12 83.2(5) . . ?
O50 Mo3 O19 167.0(6) . . ?
O29 Mo3 O19 86.7(6) . . ?
O21 Mo3 O19 83.9(6) . . ?
O24 Mo3 O19 72.9(5) . . ?
O12 Mo3 O19 75.7(5) . . ?
O22 Mo4 O14 101.6(8) . . ?
O22 Mo4 O13 99.7(7) . . ?
O14 Mo4 O13 101.0(7) . . ?
O22 Mo4 O30 101.2(8) . . ?
O14 Mo4 O30 95.3(7) . . ?
O13 Mo4 O30 150.3(6) . . ?
O22 Mo4 O20 87.6(7) . . ?
O14 Mo4 O20 170.6(7) . . ?
O13 Mo4 O20 79.1(6) . . ?
O30 Mo4 O20 80.9(6) . . ?
O22 Mo4 O21 166.9(7) . . ?
O14 Mo4 O21 90.7(7) . . ?
O13 Mo4 O21 73.4(6) . . ?
O30 Mo4 O21 81.8(6) . . ?
O20 Mo4 O21 80.3(6) . . ?
O22 Mo4 V3 132.0(6) . . ?
O14 Mo4 V3 101.3(5) . . ?
O13 Mo4 V3 34.4(4) . . ?
O30 Mo4 V3 118.0(5) . . ?
O20 Mo4 V3 73.4(4) . . ?
O21 Mo4 V3 39.3(4) . . ?
O22 Mo4 Cs3 55.0(6) . . ?
O14 Mo4 Cs3 140.9(5) . . ?
O13 Mo4 Cs3 112.8(5) . . ?
O30 Mo4 Cs3 64.5(5) . . ?
O20 Mo4 Cs3 44.4(4) . . ?
O21 Mo4 Cs3 116.8(4) . . ?
V3 Mo4 Cs3 117.65(11) . . ?
O31 Mo5 O32 104.5(9) . . ?
O31 Mo5 O26 101.4(7) . . ?
O32 Mo5 O26 98.6(8) . . ?
O31 Mo5 O33 96.9(7) . . ?
O32 Mo5 O33 99.2(7) . . ?
O26 Mo5 O33 150.3(6) . . ?
O31 Mo5 O28 164.3(7) . . ?
O32 Mo5 O28 89.1(7) . . ?
O26 Mo5 O28 84.0(6) . . ?
O33 Mo5 O28 72.7(6) . . ?
O31 Mo5 O27 85.2(7) . . ?
O32 Mo5 O27 170.2(7) . . ?
O26 Mo5 O27 77.7(6) . . ?
O33 Mo5 O27 80.8(6) . . ?
O28 Mo5 O27 81.6(5) . . ?
O31 Mo5 Cs3 154.5(6) . . ?
O32 Mo5 Cs3 51.3(6) . . ?
O26 Mo5 Cs3 77.8(5) . . ?
O33 Mo5 Cs3 95.2(5) . . ?
O28 Mo5 Cs3 40.9(4) . . ?
O27 Mo5 Cs3 118.9(4) . . ?
O34 Mo6 O35 103.8(8) . . ?
O34 Mo6 O30 99.4(8) . . ?
O35 Mo6 O30 102.7(7) . . ?
O34 Mo6 O33 99.6(7) . . ?
O35 Mo6 O33 96.1(7) . . ?
O30 Mo6 O33 149.1(6) . . ?
O34 Mo6 O28 89.9(7) . . ?
O35 Mo6 O28 163.5(7) . . ?
O30 Mo6 O28 83.7(6) . . ?
O33 Mo6 O28 72.2(6) . . ?
O34 Mo6 O29 171.4(7) . . ?
O35 Mo6 O29 84.8(7) . . ?
O30 Mo6 O29 77.5(6) . . ?
O33 Mo6 O29 80.2(6) . . ?
O28 Mo6 O29 81.8(5) . . ?
O34 Mo6 Cs3 50.8(6) . . ?
O35 Mo6 Cs3 151.4(6) . . ?
O30 Mo6 Cs3 73.4(5) . . ?
O33 Mo6 Cs3 100.7(5) . . ?
O28 Mo6 Cs3 44.9(4) . . ?
O29 Mo6 Cs3 120.7(4) . . ?
O7 V1 O4 107.1(7) . . ?
O7 V1 O10 99.5(7) . . ?
O4 V1 O10 102.0(7) . . ?
O7 V1 O11 98.7(7) . . ?
O4 V1 O11 93.1(6) . . ?
O10 V1 O11 151.7(6) . . ?
O7 V1 O17 113.5(7) . . ?
O4 V1 O17 139.0(6) . . ?
O10 V1 O17 78.0(6) . . ?
O11 V1 O17 75.0(6) . . ?
O7 V1 Mo1 117.0(5) . . ?
O4 V1 Mo1 119.8(5) . . ?
O10 V1 Mo1 34.9(4) . . ?
O11 V1 Mo1 117.0(4) . . ?
O17 V1 Mo1 44.2(4) . . ?
O8 V2 O5 107.2(7) . . ?
O8 V2 O11 109.1(7) . . ?
O5 V2 O11 108.0(7) . . ?
O8 V2 O12 109.7(7) . . ?
O5 V2 O12 112.5(7) . . ?
O11 V2 O12 110.3(6) . . ?
O8 V2 Cs1 41.1(5) . 2_675 ?
O5 V2 Cs1 66.2(4) . 2_675 ?
O11 V2 Cs1 117.7(4) . 2_675 ?
O12 V2 Cs1 129.7(5) . 2_675 ?
O8 V2 Cs3 35.5(5) . 3_565 ?
O5 V2 Cs3 136.2(5) . 3_565 ?
O11 V2 Cs3 78.9(5) . 3_565 ?
O12 V2 Cs3 104.4(5) . 3_565 ?
Cs1 V2 Cs3 72.37(10) 2_675 3_565 ?
O9 V3 O6 107.0(7) . . ?
O9 V3 O13 101.8(7) . . ?
O6 V3 O13 100.6(7) . . ?
O9 V3 O12 102.0(7) . . ?
O6 V3 O12 90.7(6) . . ?
O13 V3 O12 149.3(6) . . ?
O9 V3 O21 106.8(7) . . ?
O6 V3 O21 145.3(7) . . ?
O13 V3 O21 79.7(6) . . ?
O12 V3 O21 75.0(6) . . ?
O9 V3 Mo4 112.3(5) . . ?
O6 V3 Mo4 124.5(5) . . ?
O13 V3 Mo4 34.8(4) . . ?
O12 V3 Mo4 116.6(4) . . ?
O21 V3 Mo4 45.2(4) . . ?
O8 Cs1 O9 95.4(4) 2_674 1_554 ?
O8 Cs1 O7 75.2(4) 2_674 . ?
O9 Cs1 O7 137.3(4) 1_554 . ?
O8 Cs1 O10 119.1(4) 2_674 . ?
O9 Cs1 O10 141.5(4) 1_554 . ?
O7 Cs1 O10 49.9(4) . . ?
O8 Cs1 O34 71.6(4) 2_674 4_554 ?
O9 Cs1 O34 117.7(4) 1_554 4_554 ?
O7 Cs1 O34 99.0(4) . 4_554 ?
O10 Cs1 O34 90.9(4) . 4_554 ?
O8 Cs1 O5 45.2(3) 2_674 2_674 ?
O9 Cs1 O5 79.1(3) 1_554 2_674 ?
O7 Cs1 O5 64.7(3) . 2_674 ?
O10 Cs1 O5 112.4(3) . 2_674 ?
O34 Cs1 O5 116.5(4) 4_554 2_674 ?
O8 Cs1 O16 148.4(4) 2_674 . ?
O9 Cs1 O16 95.1(4) 1_554 . ?
O7 Cs1 O16 76.8(3) . . ?
O10 Cs1 O16 46.6(4) . . ?
O34 Cs1 O16 127.8(4) 4_554 . ?
O5 Cs1 O16 108.4(3) 2_674 . ?
O8 Cs1 V2 20.7(3) 2_674 2_674 ?
O9 Cs1 V2 86.5(3) 1_554 2_674 ?
O7 Cs1 V2 70.1(3) . 2_674 ?
O10 Cs1 V2 119.6(3) . 2_674 ?
O34 Cs1 V2 92.3(3) 4_554 2_674 ?
O5 Cs1 V2 24.58(19) 2_674 2_674 ?
O16 Cs1 V2 131.5(3) . 2_674 ?
O8 Cs1 Cs3 35.1(3) 2_674 4_554 ?
O9 Cs1 Cs3 91.5(3) 1_554 4_554 ?
O7 Cs1 Cs3 101.6(3) . 4_554 ?
O10 Cs1 Cs3 126.4(3) . 4_554 ?
O34 Cs1 Cs3 44.0(3) 4_554 4_554 ?
O5 Cs1 Cs3 77.9(2) 2_674 4_554 ?
O16 Cs1 Cs3 171.7(3) . 4_554 ?
V2 Cs1 Cs3 53.91(7) 2_674 4_554 ?
O35 Cs2 O2 90.6(5) . 4_545 ?
O35 Cs2 O14 98.4(5) . . ?
O2 Cs2 O14 60.9(4) 4_545 . ?
O35 Cs2 O30 52.3(4) . . ?
O2 Cs2 O30 79.0(4) 4_545 . ?
O14 Cs2 O30 48.1(4) . . ?
O35 Cs2 O29 52.2(4) . . ?
O2 Cs2 O29 125.7(4) 4_545 . ?
O14 Cs2 O29 84.5(4) . . ?
O30 Cs2 O29 47.6(4) . . ?
O35 Cs2 O21 87.5(4) . . ?
O2 Cs2 O21 107.3(4) 4_545 . ?
O14 Cs2 O21 47.7(3) . . ?
O30 Cs2 O21 45.6(3) . . ?
O29 Cs2 O21 44.6(3) . . ?
O35 Cs2 O50 94.5(4) . . ?
O2 Cs2 O50 151.1(4) 4_545 . ?
O14 Cs2 O50 90.1(4) . . ?
O30 Cs2 O50 81.7(3) . . ?
O29 Cs2 O50 44.5(3) . . ?
O21 Cs2 O50 44.7(3) . . ?
O35 Cs2 S2 84.0(3) . 4_545 ?
O2 Cs2 S2 16.1(3) 4_545 4_545 ?
O14 Cs2 S2 76.5(3) . 4_545 ?
O30 Cs2 S2 86.5(3) . 4_545 ?
O29 Cs2 S2 128.8(3) . 4_545 ?
O21 Cs2 S2 121.4(2) . 4_545 ?
O50 Cs2 S2 166.1(3) . 4_545 ?
O35 Cs2 Na1 112.1(4) . 3_565 ?
O2 Cs2 Na1 157.2(4) 4_545 3_565 ?
O14 Cs2 Na1 115.5(3) . 3_565 ?
O30 Cs2 Na1 116.4(3) . 3_565 ?
O29 Cs2 Na1 73.7(3) . 3_565 ?
O21 Cs2 Na1 77.4(3) . 3_565 ?
O50 Cs2 Na1 34.9(3) . 3_565 ?
S2 Cs2 Na1 156.83(16) 4_545 3_565 ?
O41 Cs3 O43 99.0(8) . . ?
O41 Cs3 O8 105.7(6) . 3_465 ?
O43 Cs3 O8 127.2(7) . 3_465 ?
O41 Cs3 O28 103.2(6) . . ?
O43 Cs3 O28 92.3(7) . . ?
O8 Cs3 O28 124.9(4) 3_465 . ?
O41 Cs3 O42 52.4(7) . . ?
O43 Cs3 O42 47.8(7) . . ?
O8 Cs3 O42 141.4(5) 3_465 . ?
O28 Cs3 O42 93.0(5) . . ?
O41 Cs3 O25 85.9(6) . 3_465 ?
O43 Cs3 O25 49.0(7) . 3_465 ?
O8 Cs3 O25 86.8(4) 3_465 3_465 ?
O28 Cs3 O25 141.3(4) . 3_465 ?
O42 Cs3 O25 62.7(5) . 3_465 ?
O41 Cs3 O24 57.3(6) . 3_465 ?
O43 Cs3 O24 97.3(7) . 3_465 ?
O8 Cs3 O24 61.7(4) 3_465 3_465 ?
O28 Cs3 O24 159.3(5) . 3_465 ?
O42 Cs3 O24 80.3(5) . 3_465 ?
O25 Cs3 O24 51.2(4) 3_465 3_465 ?
O41 Cs3 O20 56.8(6) . . ?
O43 Cs3 O20 97.3(7) . . ?
O8 Cs3 O20 135.3(4) 3_465 . ?
O28 Cs3 O20 46.4(4) . . ?
O42 Cs3 O20 64.7(5) . . ?
O25 Cs3 O20 127.1(4) 3_465 . ?
O24 Cs3 O20 113.9(4) 3_465 . ?
O41 Cs3 O34 117.8(6) . . ?
O43 Cs3 O34 132.6(7) . . ?
O8 Cs3 O34 72.4(4) 3_465 . ?
O28 Cs3 O34 52.7(4) . . ?
O42 Cs3 O34 143.7(5) . . ?
O25 Cs3 O34 151.6(4) 3_465 . ?
O24 Cs3 O34 127.0(4) 3_465 . ?
O20 Cs3 O34 81.0(4) . . ?
O41 Cs3 O18 81.5(6) . . ?
O43 Cs3 O18 58.0(7) . . ?
O8 Cs3 O18 169.1(4) 3_465 . ?
O28 Cs3 O18 44.4(4) . . ?
O42 Cs3 O18 49.5(5) . . ?
O25 Cs3 O18 102.1(4) 3_465 . ?
O24 Cs3 O18 129.0(4) 3_465 . ?
O20 Cs3 O18 42.4(4) . . ?
O34 Cs3 O18 97.1(4) . . ?
O41 Cs3 P1 79.9(6) . . ?
O43 Cs3 P1 82.8(6) . . ?
O8 Cs3 P1 146.6(4) 3_465 . ?
O28 Cs3 P1 27.0(3) . . ?
O42 Cs3 P1 67.9(4) . . ?
O25 Cs3 P1 126.6(3) 3_465 . ?
O24 Cs3 P1 136.7(3) 3_465 . ?
O20 Cs3 P1 25.5(3) . . ?
O34 Cs3 P1 76.0(3) . . ?
O18 Cs3 P1 25.1(3) . . ?
O41 Cs3 O32 153.3(6) . . ?
O43 Cs3 O32 80.7(7) . . ?
O8 Cs3 O32 95.0(4) 3_465 . ?
O28 Cs3 O32 50.4(4) . . ?
O42 Cs3 O32 117.5(5) . . ?
O25 Cs3 O32 112.3(4) 3_465 . ?
O24 Cs3 O32 149.4(4) 3_465 . ?
O20 Cs3 O32 96.6(4) . . ?
O34 Cs3 O32 52.8(4) . . ?
O18 Cs3 O32 75.9(4) . . ?
P1 Cs3 O32 73.6(3) . . ?
O51 Na1 O1 167.5(9) . 4_545 ?
O51 Na1 O22 95.6(10) . . ?
O1 Na1 O22 86.1(6) 4_545 . ?
O51 Na1 O50 91.8(8) . 3_465 ?
O1 Na1 O50 100.4(6) 4_545 3_465 ?
O22 Na1 O50 94.8(7) . 3_465 ?
O51 Na1 O38 85.6(8) . . ?
O1 Na1 O38 81.9(6) 4_545 . ?
O22 Na1 O38 95.3(7) . . ?
O50 Na1 O38 169.8(7) 3_465 . ?
O51 Na1 Na3 53.5(8) . 1_556 ?
O1 Na1 Na3 115.7(6) 4_545 1_556 ?
O22 Na1 Na3 73.7(6) . 1_556 ?
O50 Na1 Na3 140.6(6) 3_465 1_556 ?
O38 Na1 Na3 42.3(6) . 1_556 ?
O51 Na1 Cs2 62.0(8) . 3_465 ?
O1 Na1 Cs2 122.4(5) 4_545 3_465 ?
O22 Na1 Cs2 142.7(6) . 3_465 ?
O50 Na1 Cs2 59.4(4) 3_465 3_465 ?
O38 Na1 Cs2 110.9(5) . 3_465 ?
Na3 Na1 Cs2 108.2(3) 1_556 3_465 ?
O38 Na2 O2 156.5(8) . 4_545 ?
O38 Na2 O14 81.5(7) . . ?
O2 Na2 O14 82.7(7) 4_545 . ?
O38 Na2 O3 109.2(8) . 4_545 ?
O2 Na2 O3 82.9(6) 4_545 4_545 ?
O14 Na2 O3 162.8(7) . 4_545 ?
O38 Na2 O1 81.3(7) . 4_545 ?
O2 Na2 O1 81.9(6) 4_545 4_545 ?
O14 Na2 O1 91.3(6) . 4_545 ?
O3 Na2 O1 77.5(6) 4_545 4_545 ?
O38 Na2 O15 78.1(7) . 1_556 ?
O2 Na2 O15 125.3(7) 4_545 1_556 ?
O14 Na2 O15 127.4(6) . 1_556 ?
O3 Na2 O15 69.1(5) 4_545 1_556 ?
O1 Na2 O15 131.8(7) 4_545 1_556 ?
O38 Na2 O16 100.8(7) . 1_556 ?
O2 Na2 O16 93.7(6) 4_545 1_556 ?
O14 Na2 O16 81.4(6) . 1_556 ?
O3 Na2 O16 108.8(6) 4_545 1_556 ?
O1 Na2 O16 171.9(7) 4_545 1_556 ?
O15 Na2 O16 56.2(5) 1_556 1_556 ?
O38 Na2 Mo1 94.1(6) . 1_556 ?
O2 Na2 Mo1 107.3(5) 4_545 1_556 ?
O14 Na2 Mo1 108.5(5) . 1_556 ?
O3 Na2 Mo1 84.6(4) 4_545 1_556 ?
O1 Na2 Mo1 158.9(5) 4_545 1_556 ?
O15 Na2 Mo1 28.0(4) 1_556 1_556 ?
O16 Na2 Mo1 29.2(3) 1_556 1_556 ?
O1 S1 C2 107.5(9) . . ?
O1 S1 C1 105.0(10) . . ?
C2 S1 C1 100.9(11) . . ?
O1 S1 Ru1 117.4(6) . . ?
C2 S1 Ru1 111.1(7) . . ?
C1 S1 Ru1 113.5(8) . . ?
O2 S2 C4 107.7(12) . . ?
O2 S2 C3 107.5(12) . . ?
C4 S2 C3 99.8(14) . . ?
O2 S2 Ru1 120.2(7) . . ?
C4 S2 Ru1 110.9(10) . . ?
C3 S2 Ru1 108.7(9) . . ?
O2 S2 Cs2 34.1(7) . 4_554 ?
C4 S2 Cs2 99.8(9) . 4_554 ?
C3 S2 Cs2 76.6(9) . 4_554 ?
Ru1 S2 Cs2 146.9(2) . 4_554 ?
O3 S3 C5 109.3(11) . . ?
O3 S3 C6 111.3(11) . . ?
C5 S3 C6 99.9(11) . . ?
O3 S3 Ru1 113.1(7) . . ?
C5 S3 Ru1 111.3(8) . . ?
C6 S3 Ru1 111.2(8) . . ?
O18 P1 O20 108.6(9) . . ?
O18 P1 O28 107.3(9) . . ?
O20 P1 O28 109.5(9) . . ?
O18 P1 O19 112.2(9) . . ?
O20 P1 O19 110.4(9) . . ?
O28 P1 O19 108.8(8) . . ?
O18 P1 Cs3 76.4(7) . . ?
O20 P1 Cs3 71.5(7) . . ?
O28 P1 Cs3 61.2(6) . . ?
O19 P1 Cs3 169.1(6) . . ?
S1 O1 Na1 137.0(9) . 4_554 ?
S1 O1 Na2 125.2(9) . 4_554 ?
Na1 O1 Na2 95.1(6) 4_554 4_554 ?
S2 O2 Na2 124.4(10) . 4_554 ?
S2 O2 Cs2 129.9(9) . 4_554 ?
Na2 O2 Cs2 104.7(6) 4_554 4_554 ?
S3 O3 Na2 133.5(9) . 4_554 ?
V1 O4 Ru1 149.5(9) . . ?
V2 O5 Ru1 122.2(7) . . ?
V2 O5 Cs1 89.2(5) . 2_675 ?
Ru1 O5 Cs1 148.6(5) . 2_675 ?
V3 O6 Ru1 160.5(9) . . ?
V1 O7 Cs1 109.8(6) . . ?
V2 O8 Cs3 125.5(7) . 3_565 ?
V2 O8 Cs1 118.1(7) . 2_675 ?
Cs3 O8 Cs1 108.0(4) 3_565 2_675 ?
V3 O9 Cs1 145.9(8) . 1_556 ?
V1 O10 Mo1 110.7(7) . . ?
V1 O10 Cs1 100.7(6) . . ?
Mo1 O10 Cs1 114.3(6) . . ?
V2 O11 V1 126.8(8) . . ?
V2 O11 Mo2 121.2(7) . . ?
V1 O11 Mo2 100.4(6) . . ?
V2 O12 V3 128.2(7) . . ?
V2 O12 Mo3 122.0(7) . . ?
V3 O12 Mo3 100.8(6) . . ?
V3 O13 Mo4 110.8(7) . . ?
V3 O13 Na3 114.2(8) . 1_556 ?
Mo4 O13 Na3 116.4(8) . 1_556 ?
Mo4 O14 Na2 141.7(9) . . ?
Mo4 O14 Cs2 107.0(7) . . ?
Na2 O14 Cs2 97.5(6) . . ?
Mo1 O15 Na2 102.8(8) . 1_554 ?
Mo1 O16 Na2 94.3(7) . 1_554 ?
Mo1 O16 Cs1 96.7(6) . . ?
Na2 O16 Cs1 104.4(5) 1_554 . ?
Mo2 O17 V1 110.9(7) . . ?
Mo2 O17 Mo1 141.3(8) . . ?
V1 O17 Mo1 96.1(6) . . ?
P1 O18 Mo1 133.8(9) . . ?
P1 O18 Cs3 78.5(7) . . ?
Mo1 O18 Cs3 115.9(6) . . ?
P1 O19 Mo3 127.3(8) . . ?
P1 O19 Mo2 125.4(8) . . ?
Mo3 O19 Mo2 93.0(5) . . ?
P1 O20 Mo4 133.5(9) . . ?
P1 O20 Cs3 83.0(7) . . ?
Mo4 O20 Cs3 107.3(6) . . ?
Mo3 O21 V3 110.8(7) . . ?
Mo3 O21 Mo4 140.9(7) . . ?
V3 O21 Mo4 95.5(6) . . ?
Mo3 O21 Cs2 86.3(5) . . ?
V3 O21 Cs2 149.8(6) . . ?
Mo4 O21 Cs2 84.5(4) . . ?
Mo4 O22 Na1 134.0(10) . . ?
Mo4 O22 Cs3 103.4(7) . . ?
Na1 O22 Cs3 122.2(6) . . ?
Mo3 O24 Mo2 118.7(7) . . ?
Mo3 O24 Cs3 140.5(7) . 3_565 ?
Mo2 O24 Cs3 99.9(6) . 3_565 ?
Mo2 O25 Cs3 108.7(6) . 3_565 ?
Mo5 O26 Mo1 161.6(9) . . ?
Mo2 O27 Mo5 142.6(8) . . ?
P1 O28 Mo5 128.2(9) . . ?
P1 O28 Mo6 127.4(9) . . ?
Mo5 O28 Mo6 93.7(6) . . ?
P1 O28 Cs3 91.8(7) . . ?
Mo5 O28 Cs3 109.9(6) . . ?
Mo6 O28 Cs3 102.9(5) . . ?
Mo3 O29 Mo6 142.9(8) . . ?
Mo3 O29 Cs2 99.1(6) . . ?
Mo6 O29 Cs2 83.2(4) . . ?
Mo6 O30 Mo4 162.2(9) . . ?
Mo6 O30 Cs2 92.5(6) . . ?
Mo4 O30 Cs2 99.3(6) . . ?
Mo5 O32 Na3 113.0(9) . 4_545 ?
Mo5 O32 Cs3 106.0(7) . . ?
Na3 O32 Cs3 123.7(8) 4_545 . ?
Mo6 O33 Mo5 116.2(8) . . ?
Mo6 O34 Cs1 159.3(9) . 4_545 ?
Mo6 O34 Cs3 105.9(7) . . ?
Cs1 O34 Cs3 92.7(5) 4_545 . ?
Mo6 O35 Cs2 106.7(7) . . ?
Na2 O38 Na1 96.8(8) . . ?
Na2 O38 Na3 123.9(10) . 1_556 ?
Na1 O38 Na3 100.8(9) . 1_556 ?
S1 C1 H1A 109.5 . . ?
S1 C1 H1B 109.5 . . ?
H1A C1 H1B 109.5 . . ?
S1 C1 H1C 109.5 . . ?
H1A C1 H1C 109.5 . . ?
H1B C1 H1C 109.5 . . ?
S1 C2 H2A 109.5 . . ?
S1 C2 H2B 109.5 . . ?
H2A C2 H2B 109.5 . . ?
S1 C2 H2C 109.5 . . ?
H2A C2 H2C 109.5 . . ?
H2B C2 H2C 109.5 . . ?
S2 C3 H3A 109.5 . . ?
S2 C3 H3B 109.5 . . ?
H3A C3 H3B 109.5 . . ?
S2 C3 H3C 109.5 . . ?
H3A C3 H3C 109.5 . . ?
H3B C3 H3C 109.5 . . ?
S2 C4 H4A 109.5 . . ?
S2 C4 H4B 109.5 . . ?
H4A C4 H4B 109.5 . . ?
S2 C4 H4C 109.5 . . ?
H4A C4 H4C 109.5 . . ?
H4B C4 H4C 109.5 . . ?
S3 C5 H5A 109.5 . . ?
S3 C5 H5B 109.5 . . ?
H5A C5 H5B 109.5 . . ?
S3 C5 H5C 109.5 . . ?
H5A C5 H5C 109.5 . . ?
H5B C5 H5C 109.5 . . ?
S3 C6 H6A 109.5 . . ?
S3 C6 H6B 109.5 . . ?
H6A C6 H6B 109.5 . . ?
S3 C6 H6C 109.5 . . ?
H6A C6 H6C 109.5 . . ?
H6B C6 H6C 109.5 . . ?
Mo3 O50 Na1 167.1(9) . 3_565 ?
Mo3 O50 Cs2 88.3(6) . . ?
Na1 O50 Cs2 85.7(5) 3_565 . ?
O13 Na3 O38 96.2(8) 1_554 1_554 ?
O13 Na3 O32 109.1(9) 1_554 4_554 ?
O38 Na3 O32 150.9(9) 1_554 4_554 ?
O13 Na3 Na1 75.8(6) 1_554 1_554 ?
O38 Na3 Na1 36.8(5) 1_554 1_554 ?
O32 Na3 Na1 136.2(9) 4_554 1_554 ?

_refine_diff_density_max         3.688
_refine_diff_density_min         -3.223
_refine_diff_density_rms         0.287



